advertisement

3B2v7:51c GML4:3:1 CSI 08125 Prod:Type: pp:1263ðcol:fig::NILÞ ED:Mahashankar PAGN: MK SCAN: Published as Z. Suo, Reliability of Interconnect Structures, pp. 265-324 in Volume 8: Interfacial and Nanoscale Failure (W. Gerberich, W. Yang, Editors), Comprehensive Structural Integrity (I. Milne, R.O. Ritchie, B. Karihaloo, Editors-in-Chief), Elsevier, Amsterdam, 2003. SX0005 8.7 Reliability of Interconnect Structures Z. SUO Mechanical and Aerospace Engineering Department and Princeton Materials Institute, Princeton University, NJ, USA 8.7.1 INTRODUCTION 2 8.7.2 CRACKING 4 8.7.2.1 8.7.2.2 8.7.2.3 8.7.2.4 8.7.2.5 8.7.2.6 8.7.2.7 Linear Elastic Fracture Mechanics On Applying Fracture Mechanics to the Interconnect Structure Energy Release Rate Channel Cracks in a Thin Film Bonded to a Substrate Measuring Thin Film Toughness The Effect of Underlayer on Channel Crack Crack Kinetics: Subcritical Cracking and Substrate Creep 8.7.3 DEBONDING AND MIXED MODE CRACK 8.7.3.1 8.7.3.2 8.7.3.3 8.7.3.4 15 16 19 21 25 Mixed Mode Crack in a Homogeneous Material Interfacial Fracture Mechanics Measuring Interfacial Fracture Energy Effects of Plasticity 8.7.4 RATCHETING 8.7.4.1 8.7.4.2 8.7.4.3 8.7.4.4 8.7.4.5 8.7.4.6 26 Temperature Cycling as a Qualiﬁcation Test Ratcheting toward a Steady State Shakedown vs Cyclic Plastic Deformation Ratcheting Strain Rate The Transient Process to Approach the Steady State Ratcheting-induced Crack Growth 8.7.5 STRESS-INDUCED VOIDING 8.7.5.1 8.7.5.2 8.7.5.3 8.7.5.4 8.7.5.5 8.7.5.6 27 29 32 34 36 38 38 Stress-Induced Voiding in Encapsulated Metal Line An Analysis of Stress-Induced Voiding Nonhydrostatic Stress State in Encapsulated Metal Line Voiding in Blanket Copper Film Slit-like Voids The Effects of Low-k Dielectrics and Barriers 8.7.6 ELECTROMIGRATION 8.7.6.1 8.7.6.2 8.7.6.3 8.7.6.4 8.7.6.5 8.7.6.6 8.7.6.7 8.7.6.8 5 6 7 9 10 12 14 39 40 44 47 47 49 51 Electromigration in Encapsulated Metal Line Basic Electromigration Characteristics Balancing Electron Wind with Stress Gradient No-Voiding Condition for Encapsulated Line Saturated Void Volume (SVV) Experimental Determination of Z ; DaðT T0 Þ; B; and D No-Extrusion Condition for Encapsulated Line The Immortal Interconnect 1 52 53 55 56 57 58 59 60 CSI : 08125 2 8.7.1 SX0010 SX0015 Reliability of Interconnect Structures INTRODUCTION On January 23, 1959, Robert Noyce wrote in his lab notebook: ‘‘yit would be desirable to make multiple devices on a single piece of silicon, in order to be able to make interconnections between devices as part of the manufacturing process, and thus reduce size, weight, etc. as well as cost per active device.’’ With these words, the co-inventor (with Jack Kilby) of the integrated circuit, and the cofounder (with Gordon Moore) of Intel Corporation a decade later, spelled out the Monolithic Idea that would shape the microelectronic revolution (bib99 Reid, 1984). To function, transistors, capacitors, and resistors must connect among themselves and to the external world. Rather than ﬁrst making these components individually and then connecting them with wires, the microelectronic technology fabricates the interconnect structure, as well as all the components, into a single solid piece, the chip. Ever since, the technology has advanced by miniaturization, squeezing more and more transistors on every single chip. By necessity the interconnect structure has complex architectures, diverse materials, and small feature sizes. Figure 1 shows a transmission electron microscope image of an interconnect structure. The structure is a three-dimensional network of conductor lines embedded in a dielectric matrix, fabricated on the silicon surface that contains the active devices. The conductor lines are on several levels, and linked by vias. The lines have rectangular cross-sections and, on a given level, have a constant thickness but variable widths. A silicon nitride ﬁlm caps the interconnect structure, serving as a barrier of the environmental molecules. Lithographically deﬁned feature sizes, such as linewidth and via size, are as small as 100 nm. Films as thin as a few nanometers are used. Traditional interconnect structures use aluminum as the conductor, and silica as the dielectric. Tungsten vias link the lines between the levels, and titanium nitride thin layers lie between the aluminum lines and the dielectric. To make faster devices, the conductor must have higher conductivity, and the dielectric must have lower dielectric constant. Copper has been used as the conductor lines in more recent interconnect structures (bib104 Rosenberg et al., 2000). The conductor lines at different levels are linked with copper vias. Liners such as tantalum lie between the conductor and the dielectric to prevent copper diffusion into the dielectric and to promote adhesion. Low-dielectric-constant materials of current use include an organic material known as SiLK (bib88 Martin et al., 2000), and a carbon doped oxide. The former is ductile, and Figure 1 A transmission electron microscope image of a cross-section of an interconnect structure (courtesy of John Mardinly, Intel Corporation). SX0020 CSI : 08125 Introduction SX0025 SX0030 SX0035 the latter is brittle. Both are compliant compared to silicon dioxide. To further reduce the dielectric constant, other materials, including porous materials, will be used in future interconnects (bib93 Morgen et al., 1999). The Monolithic Idea solves one problem, but creates another. Making reliable interconnect structures has been a persistent challenge. Stress results from material deposition, thermal expansion mismatch, and electromigration. Material deposition inevitably generates stress; e.g., deposition of refractory metals such as tungsten usually generates stress in the GPa range. Materials in interconnect structures, selected to function as conductors, dielectrics, or barriers, have dissimilar thermal expansion coefﬁcients. On cooling from the fabrication temperature, the structures acquire stresses. To ﬁt into the small space, each conductor line must have a small cross-sectional area. The intense electric current motivates metal atoms to diffuse in the line, generating tension where atoms deplete, and compression where atoms accumulate. The study of interconnect reliability has a long history. Electromigration has been a persistent concern ever since integrated circuits were mass-produced (bib16 Blech and Meieran, 1967). As atoms diffuse, voids grow and sever metal lines. Stress-induced voiding was observed in the 1980s, when the technology brought the linewidth comparable to the line thickness (bib24 Curry et al., 1984). Such an aluminum line, of approximately square crosssection, encapsulated in silica, develops triaxial stresses of magnitude much above the yield strength of aluminum (bib64 Jones and Basehore, 1987). Voids grow to relax the stresses, facilitated by atomic diffusion (bib106 Sauter and Nix, 1992; bib69 Korhonen et al., 1993). Around the same time, thin ﬁlm fracture mechanics was advanced (bib30 Evans et al., 1988; bib61 Hutchinson and Suo, 1991; bib124 Thouless, 1991), providing tools to quantify toughness of thin ﬁlms (bib85 Ma et al., 1998; bib23 Cook and Liniger, 1999), and adhesion between thin ﬁlms (bib25 Dauskardt et al., 1998; bib132 Volinsky et al., 2002). The tools have been incorporated into industrial practice in material selection, process control, and failure analysis. More recently, a new failure mechanism has been identiﬁed, in which cracks grow in brittle ﬁlms under cyclic temperatures, aided by ratcheting deformation in a metal underlayer (bib57 Huang et al., 2000). Stress-induced voiding has been observed in blanket copper ﬁlms (bib109 Shaw et al., 2001; bib107 Sekiguchi et al., 2001), and in copper vias in the copper/silica interconnect structure (bib47 3 Hommel et al., 2001; bib96 Ogawa et al., 2002). Low dielectric constant materials have low stiffness; their effects on interconnect reliability are the focus of current studies (bib75 Lee et al., 2002; bib4 Ambrico et al., 2002; bib78 bib79 Liang et al., 2002a, 2002b; bib102 Rim et al., 2002). This chapter is organized according to failure modes: cracking, debonding, ratcheting, voiding, and electromigration. Such perversities are not only nuisances—problems to be tested away by trial-and-error, but also opportunities for fundamental study of the mechanical behavior of diverse materials, in integrated structures, at an unprecedented small size scale. The study of electromigration has led to the discovery that adding a few percent of copper into aluminum interconnects slows aluminum diffusion rate by nearly two orders of magnitude. As of early 2000s, the atomistic origin of this behavior is still not fully understood. The observation of stress-induced voiding, perhaps more than any other single event, has motivated academic researchers to join their industrial colleagues to study atomistic processes of stress generation and relaxation in thin ﬁlms. The introduction of copper and lowdielectric-constant materials has given a new urgency to study cracking and debonding in small structures. The fundamental study will impact other major technologies, such as MEMS, integrated photonics, and thermal barrier coatings, where small-structure mechanical behavior is important. bib131 Vinci and Baker (2002) have edited a multi-author review on mechanical properties in small dimensions. The present (our context is early 2000s) method to design reliable small structures, if there is one, rests on continuum mechanics, manifest in handbook solutions, commercial ﬁnite element codes, and related measurement protocols. Their inadequacy is increasingly evident when the structures become small, because (among other issues) plastic ﬂows become discrete, and failure phenomena become nucleation, rather than growth, controlled. In the rapidly changing economics of tools for the small, the division of labor has yet been settled: what to understand, what to compute, and what to measure. The tension between the relentless trend of miniaturization and the disquieting lack of a method to design for reliability will inspire innovations for years to come. SX0040 SX0045 CSI : 08125 4 8.7.2 SX0050 SX0055 SX0060 Reliability of Interconnect Structures CRACKING Figure 2 illustrates cracks in a brittle thin ﬁlm bonded on a silicon substrate. The ﬁlm is under a state of biaxial tensile stress. Starting from a ﬂaw in the ﬁlm, a crack runs across the ﬁlm thickness and often arrests at the interface, leaving the interface and the substrate intact. The crack, however, elongates laterally in the ﬁlm, uninhibited until it meets a ﬁlm edge or another crack. The lateral crack length can be many times the ﬁlm thickness. Such a crack is known as a channel crack. Because the ﬁlm may have many pre-existing ﬂaws, under a large stress, many channel cracks can form. A cracked ﬁlm looks like a ﬁeld of drying mud. A brittle material fractures by breaking atomic bonds along the front of a crack. The atomistic bond-breaking process remains unchanged when this brittle material is integrated in a structure, surrounded by other materials, so long as the feature size is large compared to individual atoms. It is, however, the close proximity of the dissimilar materials that gives rise to the diverse fracture behaviors observed in the interconnect structure. The integration of dissimilar materials introduces stresses. During fracture, even when the crack is conﬁned in the brittle material, the surrounding materials deform, sometimes inelastcially. The pragmatic approach to fracture in the interconnect structure pays little attention to the atomistic bond-breaking process itself, but instead focuses on deformation in the surrounding materials. The division of labor is brilliantly made within the framework of linear elastic fracture mechanics: (a) The fracture toughness is a property speciﬁc to the given brittle material, unaffected by the surrounding materials, and is measured experimentally. (b) The crack driving force depends on the surrounding materials, and is related to their deformation by calculation. We begin with an outline of the linear elastic fracture mechanics, and its use in the interconnect structure. Energy consideration is taken up next. We then describe a channel crack in a thin ﬁlm bonded to an elastic substrate. This simple structure leads to a method to measure the fracture toughness. To illustrate the effects of deformation, we examine a channel crack in a brittle ﬁlm on an inelastic underlayer. The crack velocity is set by creep in the underlayer, as well as by subcritical cracking in the brittle ﬁlm. 8.7.2.1 SX0061 Linear Elastic Fracture Mechanics bib74 Lawn (1993) is an established textbook on brittle fracture. Here we outline the fundamentals of immediate importance to the interconnect structure. Figure 3 illustrates a crack in a body subject to a distribution of load that opens the crack. Model the body by a linear elastic solid, the crack faces by two matching surfaces, and the crack front by a curve. Within the theory of linear elasticity, a boundary value problem determines the stress ﬁeld in the body. Of course, the stress ﬁeld depends on the boundary conditions: the size and the shape of the crack and the body, as Figure 2 A plan view of a silicon nitride ﬁlm of B1 mm thickness grown on a silicon substrate. The tensile stress in the ﬁlm causes channel cracks. The contrast indicates that the ﬁlm also partially debonds from the substrate (courtesy of Q. Ma, Intel Corporation). SX0065 CSI : 08125 Cracking Figure 3 A crack in a body subject to a distribution of load that opens the crack. Also shown is the coordinate system in a plane normal to the crack front. SX0070 well as the magnitude and the distribution of the load. By modeling the crack front as a mathematical curve, the linear elasticity theory does not account for the atomistic bondbreaking process. One feature of the stress ﬁeld, common to all such elasticity boundary value problems, plays a special role in the fracture mechanics. Let (r, y) be the polar coordinates, centered at a particular point along the crack front, in the plane normal to the crack front. The (x1, x2) coordinates are in the same plane. The linear elasticity theory shows that the stress ﬁeld in the body takes the form K sij ðr; yÞ ¼ pﬃﬃﬃﬃﬃﬃﬃ Sij ðyÞ: 2pr ð1Þ The dependence on r is square-root singular. The stress ﬁeld scales with K, known as the stress intensity factor. The factor 2p is introduced by convention. The y-dependent functions, Sij(y), are listed in bib74 Lawn (1993); for example, S22 ðyÞ ¼ cos ðy=2Þ½1 þ sin ðy=2Þsin ð3y=2Þ: ð2Þ The opening stress a distance r directly ahead of the crack front is K s22 ðr; 0Þ ¼ pﬃﬃﬃﬃﬃﬃﬃ: 2pr SX0075 ð3Þ For a crack in three dimensions, the stress intensity factor K may vary along the front of the crack. The r- and y-dependence of the singular stress ﬁeld are independent of the boundary 5 Figure 4 The singular stress ﬁeld is valid in the Kannulus. Inside the inner circle, the atomistic bondbreaking process invalidates the linear elasticity theory. Outside the outer circle, the boundary conditions invalidate the singular stress ﬁeld. conditions. The boundary conditions, however, do determine the magnitude of the stress intensity factor K. For example, a crack of length 2a, in an inﬁnite elastic sheet, subject to a tensile stress s remote frompthe ﬃﬃﬃﬃﬃﬃ crack, has the stress intensity factor K ¼ s pa: Solutions of the stress intensity factors for many crack conﬁgurations are collected in handbooks (e.g., bib122 Tada et al., 1985). Commercial ﬁnite element codes are routinely used to calculate K for complex crack conﬁgurations. Dimensional considerations dictate that the stress intensity factor should take the form pﬃﬃﬃﬃ K ¼ ks L; ð4Þ where L is a representative length, s a representative stress, and k a dimensionless number. The number k is determined by solving the boundary value problem. It depends on the ratio of the crack length to L, as well as other ratios that characterize the integrated structure. Examples will be given later. As mentioned above, the theory of elasticity predicts that the stress ﬁeld is square-root singular. Of course, we do not believe that the stress is inﬁnite at the crack front. The physical signiﬁcance of the singular stress ﬁeld is understood as follows (Figure 4). Imagine the plane normal to the crack front. The stress ﬁeld (1) is valid in an annulus, with the inner radius larger than the zone in which the bond-break- SX0080 CSI : 08125 6 SX0085 SX0090 SX0091 Reliability of Interconnect Structures ing process invalidates the linear elasticity theory, and the outer radius smaller than the size of the body and the crack. We call this annulus the K-annulus. Neither the bondbreaking processes inside the inner circle, nor the boundary conditions outside the outer circle affect the r- and y-dependence of the stress ﬁeld in the K-annulus: the stress ﬁeld (1) is valid in this annulus. For a brittle solid, the bond-breaking processes invalidate the linear elasticity theory within a zone about 1 nm. A representative feature size in interconnect structures is 100 nm. These lengths roughly set the size of the K-annulus. So far the model does not account for the atomistic bond-breaking process. Imagine two samples of the same solid, each containing a crack under an opening load. The two samples may have different sizes and shapes. The loads on the two samples may also be different. Regardless of such differences, because the stress ﬁeld in the K-annulus depends on the boundary conditions through the stress intensity factor, the bond-breaking processes in the two samples must be identical if K is the same for the two samples. That is, K is the only messenger between the external boundary conditions and the bond-breaking process. The central idea of the linear elastic fracture mechanics has been so summarized: the same K, the same crack-tip process. Within the fracture mechanics, the simplest way to account for the bond-breaking process is to stipulate that the crack extends when the stress intensity factor K in a body containing a crack reaches a critical value, Kc, known as the fracture toughness. Once the stress intensity factor is calculated for a given crack conﬁguration, in the form of (4), the condition for the crack to grow is pﬃﬃﬃﬃ ks L ¼ Kc : SX0092 ð5Þ For a given material, the fracture toughness is determined experimentally. Start with a specimen of the material, introduce a crack into the sample, load the sample until the crack extends, and record the critical load. Independently solve the elasticity boundary value problem, and obtain the stress intensity factor in the form (4). The experimentally measured critical load then gives the fracture toughness. The fracture toughness is a material property, which is independent of the sample geometry and load. The stress intensity factor is a loading parameter, which does depend on the sample geometry and the load. 8.7.2.2 On Applying Fracture Mechanics to the Interconnect Structure bib82 Liu et al. (2000) have discussed the use of fracture mechanics to formulate design rules for the interconnect structure. For example, assume that the representative stress is set by the thermal mismatch between two materials. The length L can be set to be a feature size, such as ﬁlm thickness or via diameter. To compute k, one needs to place a crack in the structure, and know its location, orientation, and size. Such information is never available for a complex structure. A pragmatic approach is to place cracks in the structure hypothetically. For the interconnect structure, the fabrication process controls the structure to the feature size, so that the crack size should not exceed the feature size. Ideally, one wishes to ﬁnd the worst crack that gives the largest stress intensity factor. In practice, one does calculations for a few representative cracks. Because such an approach is time consuming, broad conclusions drawn from idealized structures are particularly valuable. To make the above discussion concrete, consider the following example (bib83 Lu et al., 1991). Figure 5 sketches the conﬁguration. A cylinder of radius R is embedded in an inﬁnite matrix. For simplicity, we assume that the cylinder and the matrix are both elastic, having similar Young’s modulus E and Poisson’s ratio n. Set the representative stress by s ¼ EDaDT=ð1 nÞ; ð6Þ where Da is the difference in the coefﬁcients of thermal expansion of the two materials, and DT the temperature change. This stress, as shown by the elasticity solution, corresponds to the magnitude of the longitudinal stress or twice that of the transverse stress in the cylinder. When the cylinder is under compression, the matrix is under a tensile hoop stress, which decays far away from the interface. We place a crack in the matrix, and ask if this crack will grow. It is sensible to place the crack near the interface and in the radial direction, where the stress is tensile and has a large magnitude. The choice of the crack length requires some thought. When the crack length approaches zero, the stress intensity factor vanishes. When the crack length approaches inﬁnity, the stress intensity factor also vanishes, because of the decaying stress ﬁeld. Figure 5 sketches the trend of the stress intensity factor as a function of the crack length. This elasticity boundary value problem has been solved analytically, giving the stress intensity factor: SX0095 SX0100 CSI : 08125 Cracking 7 Figure 5 A cylinder is embedded in a matrix. The cylinder is under compression. The tensile hoop stress in the matrix causes cracking. The stress intensity factor is plotted as a function of the crack length. p1=2 a K a 3=2 pﬃﬃﬃﬃ ¼ 1þ : 8 R R s R SX0105 If we can estimate the largest ﬂaw size possible due to a certain fabrication process, we can set the crack size to this ﬂaw size, and then calculate the stress intensity factor. If we know nothing about the ﬂaw, we may proceed as follows. The stress intensity (7) attains pﬃﬃﬃfactor ﬃ a maximum, Kmax ¼ 0:24s R; at a/R ¼ 0.5. No matrix ﬂaw can grow provided this maximum stress intensity factor is below the fracture toughness, namely, 0:24 SX0106 EDaDT pﬃﬃﬃﬃ RoKc : 1n ð8Þ This condition invokes well-deﬁned quantities, and does not rely on any knowledge of the ﬂaw. Everything else being equal, a cylinder with a smaller radius is less likely to cause matrix cracking. Assuming s ¼ 1 GPa and Kc ¼ 1 MPa m1=2 ; condition (8) gives the critical radius Rc ¼ 17 mm. 8.7.2.3 SX0110 ð7Þ Energy Release Rate Additional insight is gained by analyzing the elastic energy change associated with crack extension. Once again, consider the crack, area A, in an elastic body, subject to a distribution of load that opens the crack. Let F represent the magnitude of the load, and D the displace- ment, such that when D changes by dD, the load does work F dD to the body. Let U be the elastic energy stored in the body. When the displacement varies, but the crack area remains ﬁxed, the work done by the load equals the change in the elastic energy of the body, namely, dU ¼ F dD when dA ¼ 0. The elastic energy U is represented by the area under the load–displacement curve (Figure 6(a)). Imagine two copies of the body, identical in all respect except for a small difference in the crack areas. The copy with the larger crack is more compliant and, at the same displacement, stores lower elastic energy (Figure 6(b)). Regard the elastic energy stored in the body as a function of the displacement and the crack area, U(D, A). Deﬁne energy release rate, G, as the reduction of the elastic energy associated with the crack increasing per unit area, when the external load does no work, namely, G¼ qUðD; AÞ : qA SX0115 ð9Þ The partial derivative signiﬁes that the displacement D is held ﬁxed when the crack area A varies. For a given crack conﬁguration, one can solve the elasticity boundary value problem, compute the elastic energy stored in the body, U(D, A), and then obtain the energy release rate G. The above deﬁnition is still sloppy. In general, the energy release rate varies along the crack front. Denote the curved coordinate along the crack front by s, and the energy SX0120 CSI : 08125 8 Reliability of Interconnect Structures this detail, and assume that the energy release rate is uniform along the crack front. When both the displacement and the crack area vary, the elastic energy varies according to dU ¼ F dD G dA: ð11Þ The elastic energy is a function of the displacement and the crack area, U(D, A). The load F and the energy release rate G are the differential coefﬁcients. Just as F is the force conjugate to the displacement D, the energy release rate G is the force conjugate to the crack area A. Such a force is known as a conﬁgurational force. Deﬁne the potential energy as P ¼ U–FD. Write Equation (11) in a different form: dP ¼ D dF G dA: SX0121 SX0125 ð12Þ Now the potential energy is a function of the load and the crack area, P(F,A). The displacement D and the energy release rate G are the differential coefﬁcients. Equation (12) suggests an equivalent deﬁnition of the energy release rate: G¼ qPðF ; AÞ : qA ð13Þ The partial derivative signiﬁes that the load F is held ﬁxed when the crack area A varies. When the body is linearly elastic, U ¼ FD/2 and P ¼ – U, so that (13) becomes G¼þ Figure 6 (a) When the crack is stationary in an elastic body, the load is linear in the displacement. The area under the curve represents the elastic energy stored in the body. (b) For the two copies of the elastic body, each containing a stationary crack, the body with a larger crack area (A2) has a larger compliance. release rate is a function G(s). Imagine a body subject to a ﬁxed displacement D. The elastic energy stored in the body is a function of the crack shape, as well as the crack area. Let the crack advance by a small length da, which can vary along the crack front. Associated with the change in the crack, the elastic energy stored in the body varies by dU. Deﬁne the energy release rate such that dU ¼ Z GðsÞ da ds: ð10Þ The integral extends along the entire crack front. In what follows, we will mostly overlook qUðF ; AÞ : qA ð14Þ The partial derivative signiﬁes that the load F is held ﬁxed when the crack area A varies. The sign difference in Equations (9) and (14) reﬂects a simple physical fact. When the crack area is larger, the body is more compliant, so that the body stores less elastic energy at a ﬁxed displacement, but stores more elastic energy at a ﬁxed load. It has been shown that the energy release rate relates to the stress intensity factor as G¼ K2 ; E% ð15Þ whereE% ¼ E under the plane stress condition, and E% ¼ E=ð1 n2 Þ under the plane strain conditions. Here E is Young’s modulus, and n Poisson’s ratio. Fracture mechanics has been formulated either in terms of the stress intensity factor, or the energy release rate. The two formulations are equivalent. Both contribute to the understanding of the fracture mechanics. The simplest fracture condition is that the crack advances when the energy SX0130 CSI : 08125 Cracking release rate attains a critical value, G, known as the fracture energy. Obviously, the fracture energy relates to the fracture toughness as G ¼ % Kc2 =E: 8.7.2.4 SX0135 SX0140 Channel Cracks in a Thin Film Bonded to a Substrate In an interconnect structure, often a crack runs in one material, but the neighboring material remains intact and exerts a constraint on the crack. Figure 7 illustrates two structures for comparison. In Figure 7(a), a crack of length a, in a freestanding sheet of thickness h, is subject to a tensile stress s remote from the crack. Assume that the displacement at the load point is ﬁxed, so that the load does no work when the crack extends. When the crack is introduced, the stress near the crack faces is partially relieved. The volume in which the stress relaxes scales as a2h, so that relative to the uncracked, stressed sheet, the elastic energy in the cracked sheet changes by DUB–a2hs2/E. Consequently, GBas2/E, namely, the energy release rate for a crack in a freestanding sheet increases with the crack length. Figure 7(b) illustrates a thin elastic ﬁlm bonded to an elastic substrate. When the crack length a is much larger than the ﬁlm thickness h, the stress ﬁeld in the crack wake becomes invariant as the crack extends. The volume in which the stress relaxes scales as ah2, so that the introduction of the crack changes the elastic energy by DUB ah2 s2 =Ef : The energy release rate is 9 G¼Z s2 h : E% f ð16Þ The dimensionless number Z depends on the elastic constants of the ﬁlm and the substrate. The number must be determined by solving the boundary value problem. When the thin ﬁlm and the substrate have similar elastic constants, Z ¼ 2.0. bib11 Beuth (1992) calculated the Z values for a thin ﬁlm on an inﬁnite substrate with dissimilar elastic constants. When the substrate is stiffer than the ﬁlm, Z is between 1 and 2. When the substrate is much more compliant than the ﬁlm, Z can be very large. For the channel crack, the energy release rate scales with the ﬁlm thickness, and is independent of the crack length when the crack length exceeds several times the ﬁlm thickness (bib3 Ambrico and Begley, 2002). Take Z ¼ 2, s ¼ 109 Pa, E% f ¼ 1011 Pa; and G ¼ 10 J m2. Equating the energy release rate G in (16) to the fracture energy G, we ﬁnd a critical ﬁlm thickness hc ¼ 0.5 mm. Channel cracks can propagate in ﬁlms thicker than hc, but not in ﬁlms thinner than hc. bib138 Ye et al. (1992) have shown that the channel crack energy release rate increases if the crack can dip into the substrate, or the ﬁlm and substrate can debond. bib4 Ambrico et al. (2002) have studied channel cracks multilayers with lateral patterning, with particular reference to interconnects consisting of copper and low-k dielectrics. Using the extended ﬁnite element method (XFEM), bib58 Huang et al. (2003) have studied the effects of substrate thickness and channel spacing, with particular attention to compliant substrates. Figure 7 (a) A crack in a freestanding sheet and (b) a channel crack in a thin ﬁlm bonded to a substrate. SX0145 SX0150 CSI : 08125 10 8.7.2.5 SX0155 SX0160 Reliability of Interconnect Structures Measuring Thin Film Toughness For a brittle solid, toughness is independent of the sample size, so that one may expect to extrapolate toughness measured using bulk samples to thin ﬁlms. However, thin ﬁlms used in the interconnect structure are processed under very different conditions from bulk materials, or are unavailable in bulk form at all. Consequently, it is necessary to develop techniques to measure thin ﬁlm toughness. Such a technique is attractive if it gives reliable results, and is compatible with the interconnect fabrication process. bib85 Ma et al. (1998) have developed such a technique, on the basis of channel cracks in a thin ﬁlm bonded to a silicon substrate. The test procedure consists of two steps (Figure 8): (a) generating pre-cracks, and (b) propagating the cracks using controlled stress. A convenient way of generating precracks is by scratching the surface using a sharp object. A gentle scratch usually generates multiple cracks on the two sides of the scratch. Care must be taken to generate cracks just in the ﬁlm, but not in the substrate. Use a bending ﬁxture to load the sample, and a digital camera to record the crack growth events. After a crack propagates some distance away from the scratch, the crack grows at a steady velocity. By recording crack growth at slightly different bending loads, one can measure the crack velocity as a function of the stress. The steady velocity is very sensitive to the applied stress. Consequently, the critical stress is accurately measured by controlling the velocity within a certain range that is convenient for the experiment. The critical stress then determines the fracture energy according to the mechanics result (16). The technique has been used to measure the fracture energy of silica and silicon nitride (G ¼ 16.5 J m2) (G ¼ 8.7 J m2) (bib85 Ma et al., 1998), as well as a carbon doped oxide (G ¼ 1.5 J m2) (Jun He, private communication). After deposition, the ﬁlm has a residual stress, sR. The residual stress can be measured by the wafer curvature method (bib95 Nix, 1989). When the structure is bent by a moment M (per unit thickness), the ﬁlm stress becomes s ¼ sR þ 6E% f M ; E% s Hs2 ð17Þ where Hs is the thickness of the substrate, and E% f and E% s are the plane-strain modulus of the ﬁlm and the substrate. The bending moment also causes a tensile stress in the substrate, ss ¼ 6M=Hs2 : To measure the toughness of the ﬁlm, one has to propagate the channel crack in the ﬁlm without fracturing the substrate. This, in turn, requires that the substrate should have very small ﬂaw size, and that the scratch should not produce ﬂaws in the substrate. When properly cut, the silicon substrate can sustain tensile stresses well over 1 GPa. Inspecting (16) and (17), one concludes that the technique is inapplicable when the ﬁlm has a very large fracture energy, large residual compressive Figure 8 A micrograph of cracked ﬁlm surface. Initial cracks are introduced by a scratch. When a bending load is applied, the cracks propagate in the direction normal to the bending stress. SX0165 CSI : 08125 Cracking SX0170 stress, small thickness, or low modulus. In the experiment of bib85 Ma et al. (1998), a thin metal layer is deposited on the silicon substrate, and the brittle ﬁlm is deposited on the metal. The metal layer serves as a barrier preventing the crack from entering the substrate. The metal layer, upon yielding, also increases the energy release rate for a given bending moment (Section 8.7.2.6). One may also greatly amplify the energy release rate for a given stress by using the structure in Figure 9. The cavity underneath the brittle ﬁlm may be made by MEMS fabrication method. When the crack grows, the stress in the ﬁlm is relaxed, and the energy release rate, G¼ s2 L ; E% f ð18Þ now scales with the length of the cavity, rather than the ﬁlm thickness. 8.7.2.6 SX0175 The Effect of Underlayer on Channel Crack When a brittle ﬁlm is bonded to a plastically deformable substrate, the constraint of the 11 substrate on the crack in the ﬁlm is partially lost. In the limiting case, when the yield strength of the substrate is much below the stress in the ﬁlm, the ﬁlm is equivalent to a freestanding sheet. Consequently, the plastic deformation in the substrate encourages the channel cracks in the ﬁlm. This effect has been studied by bib54 Hu and Evans (1989) by using a shear lag model, by bib12 Beuth and Klingbeil (1996) for a brittle ﬁlm on a semiinﬁnite elastic–plastic substrate, and by bib3 Ambrico and Begley (2002) for a brittle ﬁlm on a ductile underlayer. In this section, using a shear lag model, we (bib118 Suo and He, 2002) examine the structure depicted in Figure 10, consisting of an overlayer, an underlayer, and a substrate. The crack cuts across the overlayer, with the crack root arresting at the interface between the overlayer and the underlayer. The overlayer is taken to be elastic, and the substrate is rigid. The property of the underlayer will be varied to study its effect on the channel crack. The overlayer may consist of multiple brittle ﬁlms. The stress in the overlayer is a function of the position through the thickness, s(z). Deﬁne the membrane force in the overlayer by Figure 9 When the ﬁlm is above a wide cavity, the crack driving force increases greatly. Figure 10 A structure consists of an elastic overlayer, an elastic–plastic underlayer, and a rigid substrate. SX0180 CSI : 08125 12 Reliability of Interconnect Structures N¼ Z sðzÞ dz: ð19Þ The integral extends over the thickness of the overlayer. Similarly, deﬁne the membrane stiffness by B¼ SX0190 SX0191 Z % dz; EðzÞ du : dx ð22Þ Inserting (21) into (22), we obtain the ordinary differential equation for u(x): B SX0195 d2 u ¼ tðuÞ: dx2 ð23Þ Multiplying (23) by du/dx, and integrating from x ¼ 0 to x ¼ N, we obtain that 2 NN ¼ 2B Z u0 tðuÞ du: Z G dz ð25Þ gives the elastic energy change associated with the crack advancing per unit length in the overlayer. The quantity f has the unit of force, and is the driving force for the channel crack. The channel driving force is given by the complementary energy integral (bib12 Beuth and Klingbeil, 1996): f ¼2 Z SX0205 NN u0 dNN : ð26Þ 0 Once the u0–NN relation is obtained from (24), the driving force for the channel crack is calculated from (26). We next list solutions for idealized material law, t(u). We assume that the underlayer has the uniform property, and the shear stress is constant across the thickness of the underlayer. Consequently, the shear strain g is also constant across the thickness of the underlayer. The shear strain relates to the overlayer displacement as g(x) ¼ u(x)/H, where H is the thickness of the underlayer. SX0210 ð21Þ The force balance of an element of the overlayer requires that dN ¼ t: dx f ¼ SX0200 ð20Þ % where EðzÞ is the plane strain modulus of the material at z. We now consider the wake of the crack in the overlayer on a ductile underlayer. When the overlayer is uncracked, subject to a membrane force NN, uniform in the plane of the layer, the displacement ﬁeld in the overlayer is set to be zero. Relative to this reference state, the overlayer deforms when a crack is introduced. Let u(x) be the displacement ﬁeld averaged across the thickness of the overlayer. On the interface, the overlayer and the underlayer interact with each other through the shear stress ﬁeld t(x). We model the underlayer as a time-independent elastic plastic material, with a nonlinear relation between the shear stress t and the displacement u. When a crack cuts across the thickness of the overlayer at x ¼ 0, the membrane force in the overlayer, N(x), varies with the position, having the boundary conditions N(0) ¼ 0 and N(N) ¼ NN. Hooke’s law relates the membrane force to the displacement gradient: NðxÞ ¼ NN þ B the membrane force NN in the uncracked overlayer. For a multi-material overlayer, the energy release rate depends on the position, G(z). The integral ð24Þ 0 In reaching the above equation, we have used the following boundary conditions: u ¼ u0 and du/dx ¼ –NN/B at x ¼ 0, and u ¼ 0 and du/ dx ¼ 0 at x ¼ N. When the underlayer property t(u) is known, (24) provides the relation between the crack opening displacement u0 and Elastic underlayer. The underlayer is linear elastic with shear modulus m, so that t ¼ mu/H. Integrating (24), we obtain the u0–NN relation sﬃﬃﬃﬃﬃﬃ H : u0 ¼ NN mB ð27Þ Integrating (26) gives the driving force for the crack in the overlayer: sﬃﬃﬃﬃﬃﬃ H 2 f ¼ NN : mB ð28Þ This result reproduces that obtained by bib141 Xia and Hutchinson (2000). As expected, the crack driving force is quadratic in the membrane force. At a given membrane force, the crack driving force is large when the underlayer is thick and compliant. This result is applicable to, for example, a nitride passivation ﬁlm on a complaint dielectric layer. As the microelectronic industry implements low-dielectric-constant materials, with accompanying low SX0215 CSI : 08125 Cracking SX0220 stiffness, the likelihood of cracking in the brittle passivation ﬁlm will increase. Rigid, perfect plastic underlayer. Neglect elasticity of the ﬁlm, and assume that the underlayer deforms plastically at a constant stress t ¼ tY. Integrating (24), we obtain the u0–NN relation u0 ¼ 2 NN : 2BtY N3 f ¼ N: 3BtY SX0225 ð31Þ Integrating (24), we obtain the opening displacement of the crack wake 2 u0 1 1 NN ¼ þ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ : gY H 2 2 tY gY HB ð32Þ This pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ is the u0–NN relation when ﬃ NN = tY gY HB41; for smaller NN, the ﬁlm is elastic, and the u0–NN relation is given by (27). Inserting the whole u0–NN relation into (26), we ﬁnd the driving force for the crack in the overlayer: " 3 3 NN NN p ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ f ¼ 1 3BtY tY gY HB 2 # NN þ3 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ tY gY HB SX0230 ð33Þ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ When NN = tY gY HB ¼ 1; the underlayer is elastic, and ﬃ (33) recovers (28). When pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ NN = tY gY HBc1; the two terms in the bracket is negligible, and (33) recovers the result for the rigid perfect plastic case (30). Power-law plastic underlayer. Now we assume that the ﬁlm deforms according to the power law u HgY n ; ð34Þ where tY is an arbitrarily selected reference stress, and gY and n are parameters used to ﬁt experiment data. Following the same procedure as before, we obtain the u0–NN relation 2 1=ðnþ1Þ u0 ðn þ 1ÞNN ¼ ; gY H 2tY gY HB ð35Þ and the crack driving force " #1=ðnþ1Þ nþ3 2gY H ðn þ 1Þnþ2 NN f ¼ : nþ3 2BHtY gY ð30Þ This reproduces the result of bib54 Hu and Evans (1989). The crack driving force is cubic in the membrane force, inversely proportional to the underlayer yield strength, and independent of the underlayer thickness. Elastic, perfectly plastic underlayer. The ﬁlm now has the shear modulus m, the yield strength tY, and the yield strain gY ¼ tY/m. When u0ogYH, the ﬁlm is elastic, and (27) provides the u0–NN relation. When u04gYH, a segment of the ﬁlm near the crack deforms plastically, and the ﬁlm fare from the crack is still elastic. Using (27), we write the yield condition in terms of the membrane force: NN pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ 1: tY gY HB t ¼ tY ð29Þ Inserting into (26) gives driving force for the crack in the overlayer: 13 ð36Þ This equation recovers the linear elastic case Equation (28) when n ¼ 1, and the rigid perfect plastic case Equation (30) when n ¼ 0. Figure 11 plots the normalized channel ﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ driving force, f =ðHgY tY gY HBÞ; as a function of p the normalized membrane force, ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ NN = tY gY HB: As expected, for the same membrane force, the more deformable the underlayer, the larger the channel driving force. 8.7.2.7 SX0235 Crack Kinetics: Subcritical Cracking and Substrate Creep As mentioned above, the crack extends in the thin ﬁlm at some ﬁnite velocity. The magnitude of the velocity is sensitive to the stress, but in general is much below the speed of the elastic waves in the solids. Consequently, the observed crack velocity should not be an inertia effect. If the brittle solid does not creep, the time dependence originates from either the bond-breaking process, or the time-dependent deformation in the surrounding materials. Slow crack growth has been extensively studied in bulk brittle materials, where the bond-breaking process is assisted by environmental molecules, such as water molecules (bib74 Lawn, 1993). The time dependence results from the transport of the environmental molecules to the crack front, and the reaction at the crack front. The crack velocity can be measured experimentally as a function of the energy release rate. bib85 Ma et al. (1998) and bib23 Cook and Liniger (1999) have provided data for several thin ﬁlms. The measured V–G curve is sometimes ﬁt to a variety of empirical relations. One such a relation, suggested by the consideration of microscopic mechanisms, is G V ¼ V0 sinh b 1 ; Gth ð37Þ SX0240 SX0245 CSI : 08125 14 Reliability of Interconnect Structures Figure 11 The driving force for channel crack as a function of the membrane force. Several underlayer behaviors are compared: elastic, perfectly plastic, elastic–plastic, elastic–perfectly-plastic, and power law. SX0250 SX0255 where V0, Gth and b are parameters to ﬁt experimental data. I owe Dr. Jun He, of Intel Corporation, for the following idea. The V–G curve is speciﬁc to the brittle material and the environment, but is independent of the surrounding materials, if they do not prevent the environmental molecules from reaching the crack front. The V–G curve for a given material can be measured using a simple structure, such as a ﬁlm on a silicon substrate. When the brittle material is in a more complex structure, the same V–G still applies. Because the crack velocity is readily measurable, the measured crack velocity, together with the known V–G curve, determines the energy release rate. The method is accurate because the crack velocity sensitively depends on the energy release rate. As we have seen in Figure 11, the energy release rate is affected by the deformation behavior of the surrounding materials. Direct measurements of G provide a means to study the deformation behavior of the surrounding materials. The crack velocity is also affected if the surrounding materials creep. As an example, consider the structure illustrated in Figure 10 again, now assume that the underlayer is viscous (bib78 Liang et al., 2002a). Initially, the ﬁlm is in a uniform biaxial tensile stress state s. When the underlayer creeps, the stress ﬁeld in the ﬁlm relaxes in the crack wake, but intensifies around the crack tip. When the crack tip moves slowly, the crack wake has a long time to relax, and the stress intensity around the crack tip increases. When the crack tip moves rapidly, the crack wake has a short time to relax, and the stress intensity around the crack tip decreases. Consequently, the crack can attain a steady velocity, given by V ¼ 0:6 Hhs2 : ZG ð38Þ As expected, the larger the steady velocity, the smaller the energy release rate. If the ﬁlm is susceptible to subcritical crack growth, one can separately determine the V–G curve of the material, e.g., using the ﬁlm on an elastic substrate. Once the crack velocity V is measured for the ﬁlm on the viscous underlayer, one can read the energy release rate G form the V–G curve. The measured V and G, together with Equation (38), provide a means to determine the viscosity of the underlayer. 8.7.3 SX0256 DEBONDING AND MIXED MODE CRACK The interconnect structure consists of many dissimilar materials. Debonding has been a primary concern. Figure 12 is a micrograph of a thin ﬁlm debonding from a substrate. Within the linear elastic fracture mechanics, we model the debond process as a crack extending on the interface between two elastic materials. Impurities, of minute amount by volume fraction, SX0260 CSI : 08125 Debonding and Mixed Mode Crack 15 Figure 12 Debond from an edge of the ﬁlm, driven by residual tensile stress in the ﬁlm. When the debond front approaches the other edge of the ﬁlm, the debond driving force decreases, so that the debond arrests before it reaches the ﬁlm edge (courtesy of Q. Ma, Intel Corporation). SX0265 SX0270 may accumulate on the interface to a large coverage, signiﬁcantly changing the interfacial fracture energy. Adhesion sensitively depends on processing conditions, and on materials deliberately added to the interface. Measurements of the interfacial fracture energy provides tools for process control and material selection to promote adhesion in interconnect structures. It is instructive to compare a crack running on a bimaterial interface to a crack running in a homogenous, isotropic material. A crack in a homogenous, isotropic material extends along such a path that the crack tip is always under the tensile condition. Consequently, the crack tip often follows a curved path, and the fracture property of a given material is prescribed by a single quantity, the mode I fracture toughness. By contrast, the crack conﬁned on a bimaterial interface often propagates under the combined tensile and shear conditions. The fracture energy depends on the relative proportion of the tensile and shear loads. This section will begin with a discussion of a stationary, planar crack in a homogenous, isotropic material, subject to the mixed mode conditions. The crack grows to seek a mode I path. We then outline the interfacial fracture mechanics, the methods to measure the fracture energy as a function of the mode angle, and the applications to interconnect structures. We ﬁnally examine the effect of plastic deformation on debonding. 8.7.3.1 Mixed Mode Crack in a Homogeneous Material First examine a stationary, planar crack in a homogenous, isotropic material. The body is subject to a distribution of load that can both open and shear the crack. Let (r,y) be the polar coordinates centered at a given point on the crack front (Figure 13). We will consider the situation that the shear load is in the plane (r,y). The stress ﬁeld near the crack front has the form KI KII sij ðr; yÞ ¼ pﬃﬃﬃﬃﬃﬃﬃSIij ðyÞ þ pﬃﬃﬃﬃﬃﬃﬃSII ij ðyÞ: 2pr 2pr ð39Þ The y-dependent functions, SIij ðyÞ and SII ij ðyÞ; can be found in bib74 Lawn (1993). The mode I ﬁeld is symmetric with the crack plane, with SI22 ð0Þ ¼ 1 and SI12 ð0Þ ¼ 0: The mode II ﬁeld is antisymmetric with the crack plane, with II SII 22 ð0Þ ¼ 0 and S12 ð0Þ ¼ 1. In particular, the stresses on the plane y ¼ 0 a distance r ahead the crack front are KI s22 ðr; 0Þ ¼ pﬃﬃﬃﬃﬃﬃﬃ; 2pr KII s12 ðr; 0Þ ¼ pﬃﬃﬃﬃﬃﬃﬃ: 2pr ð40Þ The stress intensity factors, KI and KII, scale the amplitudes of opening and shearing loads, SX0275 CSI : 08125 16 Reliability of Interconnect Structures to the two stress intensity factors by G¼ 1 2 ðK þ KII2 Þ: E% I ð42Þ Instead of using KI and KII to represent the external loads, we use G to represent the amplitude of the loads, and c to represent the mode of the loads. Under the mixed mode conditions, upon growing, the planar crack often kinks at an angle from its original plane. The kink angle depends on the relative amount of mode II to mode I load. bib29 Erdogan and Sih (1963) showed that the experimentally measured kink angles in a plexiglass are well predicted by the criterion that the crack kinks to the plane with the maximum hoop stress. For the stationary crack, the hoop stress near the crack tip is Figure 13 A crack in a body subject to both the opening and shearing loads. SX0280 SX0285 respectively. We will be interested in situations where the crack front is under tension, rather than compression, namely, KIZ0. Once a crack conﬁguration is prescribed, the stress intensity factors KI and KII are determined by solving the elasticity boundary value problem. For example, for a crack of length 2a in an inﬁnite sheet, subject to remote tensile stress s and shear stress t,pthe ﬃﬃﬃﬃﬃﬃ two stress ¼ s pa and KII ¼ intensity factors are K I pﬃﬃﬃﬃﬃﬃ t pa: Solutions for many crack conﬁgurations have been collected in handbooks (e.g., bib122 Tada et al., 1985). Finite element methods have been used routinely to determine the stress intensity factors under the mixed mode conditions (bib77 Li et al., 1985). Again, the stress ﬁeld (39) is valid in an annulus, with the inner radius larger than the zone of the bond-breaking process, and the outer radius smaller than a length representative of the external boundary conditions. The mixed mode conditions are characterized by two loading parameters, KI and KII. The two ‘‘messengers’’ transmit the boundary conditions to the crack tip process. The relative amount of mode II to mode I is speciﬁed by the mode angle c, deﬁned by tan c ¼ KII =KI : SX0290 ð41Þ With KIZ0, the mode angle ranges between p/2rcrp/2. A pure mode I crack corresponds to c ¼ 0 and pure mode II crack to either c ¼ þ p/2 or c ¼ –p/2. The energy release rate G is still deﬁned as the elastic energy reduction as the crack extends unit area, while the load does no additional work. The energy release rate relates KI y sy y ðr; yÞ ¼ pﬃﬃﬃﬃﬃﬃﬃ cos3 2 2pr KII y 2 y sin : pﬃﬃﬃﬃﬃﬃﬃ 3cos 2 2 2pr SX0295 ð43Þ The hoop stress maximizes at an angle y*, given by y 2 tan c pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ: ¼ tan 2 1 þ 1 þ 8 tan2 c ð44Þ When KII40, c40 and the crack kinks down (i.e., y*o0). The converse is true when KIIo0. When the plane crack is pure mode I, this criterion predicts that the crack extends straight ahead. When the plane crack is pure mode II, this criterion predicts that the crack kinks at an angle y* ¼ 70.51. The moving crack tip seeks a trajectory that is locally mode I; any nonzero KII will cause the crack to deﬂect. To illustrate this point, consider two examples. It is well known that a crack in a double-cantilever beam is unstable: the crack tends to curve one way or the other (Figure 14). By symmetry, the crack on the mid-plane of the sample is pure mode I. This mode I path, however, is unstable. A crack, lying slightly off the mid-plane, has a mode II component that tends to deﬂect the crack further away from the mid-plane. As a second example, Figure 15 illustrates a thin ﬁlm spalling from an adherent substrate (bib125 Thouless et al., 1987). The ﬁlm is well bonded to the substrate, and is under a residual tensile stress. It is sometimes observed that a crack starts from the edge of the ﬁlm, dives into the substrate, and then grows parallel to the interface. In the crack wake, the residual stress in the ﬁlm is partially relieved, and the ﬁlm and a thin layer of the substrate material underneath form a composite plate, bending up. This SX0300 SX0305 CSI : 08125 Debonding and Mixed Mode Crack Figure 14 (a) A crack in a double-cantilever beam tends to curve away from the mid-plane. (b) A crack slightly away from the mid-plane has a mode II component in the direction that drives the crack further away from the mid-plane. observation is peculiar in that, were the crack to run on the ﬁlm–substrate interface, the residual stress in the ﬁlm would be fully relieved in the crack wake. Such a global energy consideration has no physical basis: it is the local process of bond breaking that selects the crack path. The experimental observation has been interpreted that the crack tip moves along a mode I trajectory. To see how this works, consider a special case that the thin ﬁlm and the substrate have similar elastic modulus. Let h be the ﬁlm thickness, and d be the depth of the crack parallel to the interface. When the crack is long compared to d, the effect of the residual stress on the crack is well described by the equivalent axial force and bending moment: P ¼ sh; M ¼ 12shðd hÞ: ð45Þ The stress intensity factors have been calculated, given by pﬃﬃﬃ 1 KI ¼ pﬃﬃﬃðPd 1=2 cos o þ 2 3Md 3=2 sin oÞ; 2 ð46aÞ pﬃﬃﬃ 1 KII ¼ pﬃﬃﬃ ðPd 1=2 sin o 2 3Md 3=2 cos oÞ; ð46bÞ 2 SX0310 with oE521. Suppose that the crack selects the depth d* by the condition that KII ¼ 0, and we obtain that d* ¼ 3.8 h. One can further conﬁrm that the mode I path is stable in that, if a parallel crack at a depth d different from d*, then KII is nonzero and is in the direction that tends to deﬂect the crack back toward the depth d*. Curved crack paths can be simulated using numerical methods. For a given crack conﬁg- 17 Figure 15 (a) Schematic of a thin ﬁlm spalling from an adherent substrate, driven by the tensile stress in the ﬁlm. The crack runs along a path parallel to the interface. (b) The effective axial force and bending moment caused by the residual stress. uration, one solves the elasticity boundary value problem, and computes the stress intensity factors KI and KII. One then advances the crack by a small length in the direction, say, set by the criterion of maximum hoop stress (Equation (44)). The path so selected should be essentially a mode I path. For a single crack tip, the precise length for each increment is unimportant, so long as it is much smaller than the representative size of the sample. To simulate simultaneous growth of multiple cracks, however, one has to know how much to advance each crack. An ingredient of time dependence has to be introduced into the model. For example, if the solid is susceptible to subcritical cracking (Section 8.7.2.7), the V– G relation provides the needed information. Once the energy release rate is calculated for every crack tip in a given conﬁguration, one advances each crack according to the kinetic law for a small time step. Similarly, one can simulate the growth of a crack in three dimensions with a curved front by advancing each point on the crack front according to the kinetic law and its local energy release rate. Because the crack extends under the mode I conditions, the V–G curve can be obtained experimentally using a specimen containing a single straight mode I crack. The regular ﬁnite element method meshes the geometry of the crack and uses a ﬁne mesh near the crack tip. When the crack grows, remeshing is required. To circumvent these difﬁculties, XFEM has been advanced (bib92 Moes et al., 1999). For the nodes around the crack tip, one adds enriching functions derived from the singular crack-tip stress ﬁeld. For nodes on the crack faces, one adds the Heaviside function to represent the displacement SX0315 CSI : 08125 18 Reliability of Interconnect Structures jump. Consequently, the mesh can be coarse near the crack tip, and the elements need not conform to the crack geometry. As the cracks grow, one updates the nodes to be enriched. No remeshing is necessary. Figure 16 shows the simulated mud-crack pattern in tensile ﬁlm bonded to a substrate (bib79 Liang et al., 2002b). 8.7.3.2 SX0320 AU:1 Interfacial Fracture Mechanics Now consider a crack on the interface between two elastic materials. Williams (1959) discovered that the singular stress ﬁeld at the interface crack tip is not square-root singular. The stresses on the interface a distance r ahead of the crack tip take the form Krie s22 þ is12 ¼ pﬃﬃﬃﬃﬃﬃﬃ: 2pr ð47Þ The numbers is used: i ¼ pﬃﬃﬃﬃﬃﬃﬃnotation of complex 1 and rie ¼ eie ln r ¼ cos ðe ln rÞ þ i sin ðe ln rÞ: The bimaterial constant e is deﬁned by e¼ 1 ð3 4n1 Þ=m1 þ 1=m2 ln ; 2p ð3 4n2 Þ=m2 þ 1=m1 ð48Þ where n is Poisson’s ratio, m the shear modulus, and the subscripts 1 and 2 refer to the two materials. The constant is bounded, |e|o(1/2p) ln 3E0.175. The stress intensity factor K is complex valued, and has the dimension K ¼ ½stress ½length1=2ie : SX0325 ð49Þ The amplitude of the stress intensity factor has the familiar dimension, |K| ¼ [stress][length]1/2. Indeed, |K| relates to the energy release rate as G¼ 1 1 1 jKj2 þ : 2 E% 1 E% 2 cosh2 ðpeÞ ð50Þ For a given crack conﬁguration, the stress intensity factor K is determined by solving the elasticity boundary value problem. Finite element method and other numerical methods have been developed to determine the stress intensity factor (Matos et al., 1990). bib61 Hutchinson and Suo (1991) have compiled solutions for layered materials. Following bib101 Rice (1988), we deﬁne the mode angle c by K ¼ jKjl ie exp ðicÞ; ð51Þ where l is an arbitrary length. To see the consequence of this deﬁnition, combine (47) and (51), yielding Figure 16 Mud-crack pattern simulated by using the XFEM. AU:2 SX0330 CSI : 08125 Debonding and Mixed Mode Crack jKj s22 þ i s12 ¼ pﬃﬃﬃﬃﬃﬃﬃ ei½cþe lnðr=lÞ : 2pr ð52Þ The ratio of the shear stress to the tensile stress is s12 =s22 ¼ tan ½c þ e lnðr=LÞ: SX0331 SX0340 AU:3 SX0345 ð53Þ When e ¼ 0, as for a crack in a homogenous material, the ratio s12/s22 is independent of the distance r in the K-annulus, and the mode angle c characterizes the relative portion of shear to tension. When ea0, the ratio s12/s22 varies with the distance r, and equals tan c at r ¼ l. The variation is not rapid, because e is small and because a logarithm is a slowly varying function. Thus, tan c approximates the ratio s12/s22 so long as r is not far from l. For a brittle interface, a natural choice is l ¼ 1 nm, representative of the bond-breaking zone size. With this choice, the mode angle c represents the relative portion of shear to tension at the size scale of bond-breaking zone. In a homogeneous material, crack faces come into contact under compression. By contrast, interface crack faces may come into contact even when the remote load has a tensile component. When the contact zone is large, one has to take into account the forces on the crack faces in solving the boundary value problem. In many situations, however, the contact zone is small compared to the overall dimension. Consequently, the K-annulus exists, with the inner radius enclosing the contact zone, as well as the bond-breaking process zone. bib101 Rice (1988) has examined the condition for small-scale contact. Williams’s elastic solution shows that the displacement jump at a distance r behind the crack tip is rﬃﬃﬃﬃﬃ 1 1 Krie 2r þ : ð54Þ % % E1 E2 2ð1 þ 2ieÞ cosh ðpeÞ p d2 þ id1 ¼ The jump in the displacement component normal to the crack faces is d2 ¼ d cos ½c þ e ln ðl=rÞ tan1 ð2eÞ; ð55Þ where d ¼ ðd21 þ d22 Þ1=2 is the magnitude of the displacement jump. If the crack is required to be open within loro100 l, the mode angle must be restricted within p=2 þ 2eocop=2 þ 2:6e; p=2 2:6eocop=2 þ 2e; for e40 for eo0 ð57Þ The number 100 is arbitrary, but the condition in (57) is insensitive to this number. When 19 e ¼ 0, the above condition simply says that the contact does not occur when the crack is under tension, which is known for homogeneous materials. As an example, consider a crack, length 2a, on the interface between two semi-inﬁnite materials, subject to remote tensile stress s and shear stress t. Write s þ it ¼ Teio, so that T is the magnitude, and o the direction, of the remote load. This elasticity boundary value problem has been solved analytically, giving the stress intensity factor (bib101 Rice, 1988) pﬃﬃﬃﬃﬃﬃ K ¼ ð1 þ 2ieÞ pað2aÞie Teio : SX0350 ð58Þ The energy release rate is obtained by inserting (58) into (50). A comparison of (51) and (58) gives the mode angle: c ¼ o þ tan1 ð2eÞ þ e ln ðl=2aÞ: ð59Þ When e ¼ 0, the mode angle c equals the angle o of the remote load. The two angles are different when ea0. Consider representative values, e ¼ –0.05, l ¼ 1 nm, and 2a ¼ 1 mm. Under remote tension, o ¼ 0, one ﬁnds that c ¼ 341, indicating a signiﬁcant shear component near the crack tip, at the size scale of bond-breaking zone. As a second example, consider the debonding of a thin ﬁlm from a substrate. A ﬁlm, thickness h, is under a tensile inplane stress s and initially bonded to the substrate. The ﬁlm may debond from the root of a channel crack, or from the edge of the ﬁlm. When the debond length exceeds several times the ﬁlm thickness, the debonding process attains a steady state, in which the energy release rate is independent of the debond length. Under the plane-strain conditions, an elementary consideration gives the energy release rate G¼ s2 h : 2E% f ð60Þ The debond crack is under the mixed mode conditions. The mode angle must be determined by solving the elasticity boundary value problem. When the ﬁlm and the substrate have similar elastic constants, the stress intensity factors are given by (46), setting P ¼ sh and M ¼ 0. The mode angle is cE521. Next, examine the effect of the modulus mismatch on the mode angle. The complex stress intensity factor is given in the form K ¼ jKjhie eio : ð61Þ The magnitude |K| relates to the energy release rate (60) through the general relation (50). The angle o depends on elastic mismatch between SX0355 CSI : 08125 20 Reliability of Interconnect Structures the ﬁlm and the substrate, ranging between 401 to 601 if the mismatch is not excessive, as tabulated in bib120 Suo and Hutchinson (1990). A comparison of (61) and (51) gives the mode angle c ¼ o þ e ln ðl=hÞ: ð62Þ For representative values, e ¼ –0.05, l ¼ 1 nm, and h ¼ 1 mm, the additional angle is e ln (l/ h) ¼ 201. 8.7.3.3 SX0360 SX0365 Figure 17 A schematic of G(c). Measuring Interfacial Fracture Energy When a debond crack extends on a bimaterial interface, mixed mode conditions usually prevail. The fracture energy is a function of the mode angle, G(c). The crack extends when the energy release rate reaches the fracture energy: G ¼ G(c). Due to elastic mismatch in the two materials, one should specify the length l in deﬁning the mode angle c. The curve G(c) has been measured for a few interface (e.g., bib19 Cao and Evans, 1989; bib133 Wang and Suo, 1990; bib80 Liechti and Chai, 1991). Figure 17 sketches the trend of the G(c) curve. The fracture energy tends to increase as mode angle approaches 7p/2. The energy cost for debond varies with the relative proportion of opening and shearing modes, because, e.g., a large amount of shear may promote more inelastic deformation in the constituent materials, or promote near-tip sliding against roughness if the interface is not perfectly ﬂat. The curve G(c) need not be symmetric with respect to c ¼ 0, because the two materials on either side of the interface are dissimilar, breaking the symmetry between co0 and c40. Many test conﬁgurations for measuring interfacial fracture energy exist. (See reviews by bib61 Hutchinson and Suo (1991), bib31 Evans and Hutchinson (1995), and bib132 Volinsky et al. (2002).) For example, the process of a tensile ﬁlm debonding from a substrate is a means to determine the interfacial fracture energy. To ensure that the crack is in the steady state, one should introduce an initial debond crack of length several times the ﬁlm thickness (bib139 Yu et al., 2001). The energy release rate (60) depends on both the ﬁlm stress and the ﬁlm thickness. One may change the ﬁlm stress by varying the temperature, or by applying a mechanical load such as pulling the substrate. One may change the ﬁlm thickness during deposition. The combination of the stress and the thickness that cause the debond crack to grow gives the fracture energy according to (60). It is often more convenient to deposit a layer of a different material to increase the energy release rate. For example, Figure 18 A thin layer of material 2 is sandwiched between two substrates of material 1, using a glue layer. A crack is on one of the interfaces. Near the crack tip, the stress ﬁeld for the interfacial crack prevails. Far away from the crack, the stress ﬁeld for a crack in the homogeneous material prevails. Cr has been used as an overlayer for its high residual stress (bib8 Bagchi et al., 1994). Thick epoxy overlayers have also been used (bib108 Shaffer et al., 1996). When an overlayer is used, one should obtain a different energy release rate expression, and introduce an initial debond crack of length several times of the combined thickness of the ﬁlm and the overlayer. A class of test methods has been particularly versatile for thin ﬁlm structures (Figure 18). Suppose one needs to measure the interfacial fracture energy of a thin ﬁlm of material 1, and a substrate of material 2. One can sandwich the thin ﬁlm between two substrates of material 1. One may use a layer of adhesive, such as epoxy, to glue the bare substrate to the one covered with the ﬁlm. The substrates are much thicker than the ﬁlm and the adhesive, so that the whole specimen is easy to load. The interfacial fracture energy can be measured if SX0370 CSI : 08125 Debonding and Mixed Mode Crack SX0375 the crack runs on the desired interface. There are several advantages of methods of this kind. First, the methods are applicable for thin ﬁlms of any thickness, and can even measure the interfacial energy between two thin ﬁlms, when they are both sandwiched. Second, because the ﬁlm is still bonded to one substrate in the crack wake, the residual stress in the ﬁlm is unrelieved, and therefore does not contribute to the energy release rate. Third, the experimental data are relatively easy to interpret, as explained below. Let us return to Figure 18. Because the substrates are much thicker than the ﬁlms, the stress ﬁeld in the substrate, far away from the ﬁlms, is unaffected by the presence of the ﬁlms, and is the same as that around a crack in a homogeneous body, given in the form (39). The load on the substrate can be represented by the two stress intensity factors KI and KII for a crack in a homogenous body. Near the crack tip, the stress ﬁeld is that of an interfacial crack (47), characterized by the complex stress intensity factor K. The energy release rate is related to both the far ﬁeld and the near-tip ﬁeld, namely, G¼ SX0380 1 2 1 1 1 jKj2 ðKI þ KII2 Þ ¼ þ : 2 E% 1 E% 2 cosh2 ðpeÞ E% 1 The energy release rate can be calculated from the homogeneous specimen, neglecting the thin ﬁlms. The mode angle, however, has to be determined by solving the boundary value problem that includes the thin ﬁlms. Let cN be the mode angle of the remote load, namely, tan cN ¼ KII/KI. The local mode angle c is deﬁned by (51) using an arbitrary length l. The local mode angle relates to the remote mode angle as c ¼ cN þ o þ e ln ðl=hÞ; SX0385 ð63Þ ð64Þ where h is the thickness of one of the ﬁlms, and o is an angle that depends on the elastic properties of the ﬁlms and the substrates, as well as the ratios between various ﬁlms. bib119 Suo and Hutchinson (1989) solved the case of a single ﬁlm between two substrates, and found that o is less than 101 provided the elastic mismatch is not too large. It is rather cumbersome to keep track of the local mode angle, especially when several ﬁlms are sandwiched, and when some of them deform plastically. A common practice has been to specify the mode angle for the sandwich specimens by the remote value cN. As an example, Figure 19 illustrates a fourpoint bend specimen. The method was intro- 21 Figure 19 Four-point bend conﬁguration. Thin ﬁlms of interest are sandwiched between two silicon substrates. On bending, crack runs on one of the interfaces. duced by bib20 Charalambides et al. (1989) and bib19 Cao and Evans (1989) to determine interfacial fracture energy, and developed by bib25 Dauskardt et al. (1998) for thin ﬁlm structures relevant for interconnects. The experimental procedure is as follows. Use two silicon wafers to sandwich ﬁlms of interest. Notch the top wafer to within a few mm of the sandwiched ﬁlms with a diamond wafering blade. Place the sample in a four-point bend ﬁxture. Record load as a function of displacement, and observe the crack propagation in an optical microscope. At a certain load, a crack initiates from the notch root, approaches the interface, and then bifurcates into two cracks to propagate on the interface. When the interface cracks are long compared to the substrate thickness, the load–displacement curve exhibits a plateau—that is, the crack reaches a steady state, in which the energy release rate is independent of the crack length. At the steady state, both the energy release rate and the mode angle are obtained analytically. As shown in Figure 20, the four-point bend conﬁguration is the superposition of two other conﬁgurations, one being pure mode I, and the other being pure mode II. The energy release rates for the two conﬁgurations can be obtained from elementary considerations. Consequently, the energy release rate for the fourpoint bend specimen is G¼ 21 M 2 ; % 3 4 EH ð65Þ SX0390 CSI : 08125 22 Reliability of Interconnect Structures Figure 20 The four-bend conﬁguration is the superposition of two other conﬁgurations, one being pure mode I, and the other being pure mode II. where M is the moment per substrate unit width, H the thickness of each substrate, and E% the plane-strain modulus of the substrates. The mode angle for the four-point bend specimen is pﬃﬃﬃﬃﬃ cN ¼ tan1 ð 3=2ÞE411: SX0395 ð66Þ Once the plateau load is measured experimentally, (65) is used to calculate the fracture energy G for the mode angle 411. Also commonly used is the double-cantilever beam specimen (bib97 Oh et al., 1987; bib67 Kook and Dauskardt, 2002). The energy release rate for the double-cantilever beam specimen of a homogenous material is found in handbooks, given by G ¼ 12 ðPaÞ2 H 2 ; 1 þ 0:677 a H 3 E% ð67Þ where a is the crack length, H the thickness of each beam, P the force per beam width, and E% the plane-strain elastic modulus. The specimen is under the mode I condition, cN ¼ 01. As discussed before, a crack in a homogenous double-cantilever beam specimen tends to curve away from the mid-plane (Figure 14). By contrast, when ﬁlms are sandwiched between the two beams, creating a weak interface, the crack will propagate along the interface. In the experiment of bib97 Oh et al. (1987), 750 nm copper ﬁlms were evaporated onto two glass substrates (of size 75 mm 25 mm 2 mm). To conﬁne crack propagation to one glass–copper interface, a layer of 10–20 nm chromium was evaporated onto one substrate prior to depositing the copper ﬁlm. The chromium layer promoted adhesion. The copper ﬁlms from the two substrates were then pressure diffusion bonded. To load the sample, aluminum arms were attached by epoxy to the ends of the specimen. The thin specimen led to high enough specimen compliance that the crack was easily arrested, permitting multiple testing of one specimen. The experimentally measured load to cause the crack to propagate rapidly gave the interfacial fracture energy according to (68). The crack on the glass–copper interface displayed subcritical growth rates spanning from B108 to 103 m s1, in the range of the energy release rates from B0.5 to 2.0 J m2. The measurements of interfacial fracture energy provide a tool for process control (Dr. Q. Ma, Intel Corporation, private communication). Many factors during the interconnect fabrication process can affect adhesion. Because debonding usually occurs after a interconnect structure is fabricated, when stresses arise from, e.g., thermal expansion mismatch. After a debond is identiﬁed, one has to modify the processing conditions, fabricate the interconnect structure again, and examine if the SX0400 AU:4 CSI : 08125 Debonding and Mixed Mode Crack SX0405 SX0410 new structure has the debond. The iteration is time consuming. Alternatively, without fabricating the whole interconnect structure, one can measure the interfacial fracture energy for the interface at question under various fabrication conditions, and then select the condition that gives an adequate interfacial fracture energy. The measurements of interfacial fracture energy also provide a tool to select materials to promote adhesion. When copper was introduced into the interconnect structure in late 1990s, new barrier layers were required to prevent copper diffusion into dielectrics, and to provide adhesion of copper to the dielectrics. The sandwiched four-point bend specimens were used to measure the interfacial fracture energy of the thin ﬁlm structures with Ta and TaN as barrier layers (bib72 Lane et al., 2000), and thereby to study the effects of interfacial chemistry, copper layer thickness, and dielectric type on adhesion. Subsequently, numerous materials of low dielectric constant have been developed to compete to be a replacement for silica in the interconnect structure. To compare these materials, a commonly accepted method is desired to measure the interfacial fracture energy. bib102 Rim et al. (2002) have evaluated adhesion of a carbon-doped oxide in thin ﬁlm structures. Interfacial cracks are often susceptible to subcritical growth under static or cyclic load. Environment strongly affects the growth rate. While the implications of subcritical debond growth for long-term reliability of the interconnect structure have not been fully understood, the fracture specimens discussed above have been used to study subcritical debond growth (bib67 Kook and Dauskardt, 2002; bib112 Snodgrass et al., 2002). 8.7.3.4 SX0415 SX0420 23 between two silicon wafers (Figure 21). The crack extends on the interface between one wafer and the brittle ﬁlm by a bond-breaking process. So long as the brittle ﬁlm thickness is large compared to the atomic spacing, the bond-breaking process is unaffected by the presence of the ductile ﬁlm. Consequently, the fracture energy G is well deﬁned for the interface between the wafer and the brittle ﬁlm. As the crack extends, a material particle in the ductile layer deforms plastically, and then unloads elastically. This hysteresis can be accounted for by the continuum theory of plasticity. In the silicon wafers, far away from the ﬁlms, the stress state is the same as that for a crack in a homogeneous elastic material, with the energy release rate G representing the amplitude of the external load. An elastic– plastic boundary value problem relates the external load G to the bond-breaking energy G and the plastic deformation properties (bib121 Suo et al., 1993; bib72 Lane et al., 2000). The hysteresis costs energy. The energy release rate Effects of Plasticity The above discussions are conﬁned in the linear elastic fracture mechanics (LEFM). One of the main requirements of the LEFM is that the inelastic zone around the crack tip must be much smaller than the feature size, in our case, the ﬁlm thickness. The inelastic deformation within the small zone is accounted for by the fracture energy. In computing the energy release rate, the structure is taken to be elastic. When the inelastic zone is large compared to the ﬁlm thickness, however, we must consider the inelastic deformation more explicitly. The following examples illustrate roles played by plasticity. As a ﬁrst example, consider two ﬁlms, one brittle and the other ductile, sandwiched Figure 21 A brittle ﬁlm and a ductile ﬁlm are sandwiched between two silicon wafers. The crack runs on the interface between one silicon wafer and the brittle ﬁlm. As the crack tip passes by, a material particle in the ductile layer undergoes a history of deformation: elastic (A), yielding (B), plastic straining (C), and elastic unloading (D). CSI : 08125 24 SX0425 Reliability of Interconnect Structures to maintain steady-state crack growth, Gss, exceeds the interfacial fracture energy G. The ratio Gss/G depends on the thicknesses of the two ﬁlms, and on the yield strength of the ductile layer. When the ductile layer is absent, Gss/G ¼ 1, so that G can be determined experimentally by the external load. By gradually increasing the ductile layer thickness, the effect of plastic deformation on Gss can be both measured and calculated. One may study deformation properties of the ductile layer this way. A second example involves a crack on a metal–ceramic interface (Figure 22). The metal deforms plastically, which may be described by the continuum plasticity theory (bib60 Hutchinson and Evans, 2000), or by dislocation dynamics (bib94 Needleman and Van der Giessen, 2001). Two classes of failure modes are envisioned. The crack may extend by decohesion (Figure 22(a)). The bond-breaking process may be characterized by a tractiondisplacement law. The crack tip is no longer a structureless point, but spreads out into a cohesive zone. The deformation hysteresis in the metal costs energy, as discussed above. Figure 22 A crack on a metal–ceramic interface. The plastic deformation may be described by continuum plasticity theory or by discrete dislocation dynamics. (a) Crack grows by a bond-breaking process. (b) Crack tip blunts, and voids open ahead of the crack tip. Alternatively, the crack may extend by linking voids (Figure 22(b)). As the load increases and the crack tip blunts, the peak stress remains constant (a few times the yield strength), but the strain keeps increasing (bib111 Shih et al., 1991). Voids open ahead of the crack tip, and link together to extend the crack. The behavior is similar to ductile fracture of bulk metals. As a third example, consider a thin metal ﬁlm sandwiched between two elastic substrates (Figure 23). A debond crack preexists on one of the interfaces. The substrates are loaded to open the crack. Let h be the ﬁlm thickness, and rp be the plastic zone size upon crack propagation. When hcrp, the substrates place no additional constraint on fracture, and the behavior is the same as described in Figure 22. When horp, however, the substrates constrain the plastic ﬂow in the ﬁlm. As the load increases and the crack tip blunts, the level of the peak stress in the metal increases, and the location of the peak stress is several times the ﬁlm thickness ahead of the crack tip (bib130 Varias et al., 1991). The high stress activates ﬂaws ahead of the crack tip into new debond areas, which link back to the main crack (bib100 Reimanis et al., 1991). When the ﬁlm thickness is very small, the dislocations emitted from the crack tip pile up at the substrate–ﬁlm interfaces (Figure 24). As the load increases and the crack tip blunts, more dislocations pile up and the stress at the crack tip can increase up to the theoretical strength (bib49 Hsia et al., 1994; bib86 Mao and Evans, Figure 23 A thin metal ﬁlm is sandwiched between two ceramic plates. The plastic deformation in the metal is constrained, leading to high triaxial stresses several ﬁlm thicknesses ahead of the crack tip. SX0430 CSI : 08125 Ratcheting 25 structure, with an aluminum ﬁlm on silica. The feature size in the interconnect structure is much smaller than the overall package. Before the die is bonded to the substrate, a silicon nitride (SiN) ﬁlm is deposited over the interconnect structure, covering both the metal and the dielectric, serving as a barrier to environmental molecules. Observed failure modes in such a package caused by temperature cycling include * * * Figure 24 A very thin metal ﬁlm is sandwiched between two ceramic plates. Dislocations emitted from the crack tip pile up at the interface. As the applied load increases, the stress at the blunted crack tip can be very high, leading to cleavage. * * 1997). Even FCC metals can fracture by cleavage this way. 8.7.4 8.7.4.1 SX0435 SX0440 RATCHETING Temperature Cycling as a Qualiﬁcation Test Temperature cycling has long been used as a test to qualify devices (bib113 Suhir, 2002). After being cycled between two temperatures, say –551C to 1251C for 1,000 times, a device is tested for its functions, and then sectioned and examined in microscopes for failure modes (e.g., distortion and cracking). If a failure mode is found, one makes a new device by modifying either processing parameters, or geometries, or materials. The new device is temperature cycled again, followed by the microscopy examination. The iterations do not guarantee quick convergence, as the modiﬁcations made to avert one failure mode may cause another. These make-and-break iterations are extremely time consuming, and are a bottleneck for innovation. Consequently, it is urgent to understand various failure modes caused by temperature cycling. Figures 25(a) and (b) are a photo of a ﬂipchip package and a schematic of its crosssection. An organic substrate is bonded to a silicon die on the face that contains transistors. The solder bumps connect the interconnects on the die to the printed circuits on the substrate. Layers of polymers (epoxy underﬁll and polyimide) lie between the substrate and the die. Figure 25(c) illustrates part of the interconnect die–polymer or polymer–substrate debonding (bib137 Yan and Agarwal, 1998; bib39 Gurumurthy et al., 1998), solder bump detachment (bib73 Lau et al., 1998), silicon die cracking (bib40 Han, 2001; bib91 Michaelides and Sitaraman, 1999), SiN ﬁlm cracking (bib57 bib56 Huang et al., 2000, 2002; bib28 Edwards et al., 1987; bib2 Alpern et al., 1994; bib36 Gee et al., 1995), and metal ﬁlm crawling (bib55 Huang et al., 2001; bib2 Alpern et al., 1994; bib62 Isagawa et al., 1980; bib123 Thomas, 1985). The last two failure modes in the above list occur in the interconnect structure, and provide the focus of the following discussion. Figure 26 shows the micrographs taken after temperature cycles. Figure 26(a) is a plan view of the die surface near a corner of a test structure. The structure has many aluminum pads. Cracks develop in the SiN ﬁlm over some of the aluminum pads. Figure 26(b) shows a patterned aluminum pad on silica, with a SiN ﬁlm covering both aluminum and silica. Cracks form in SiN over aluminum, but not in SiN over silica. Figure 26(c) shows a cross-section of a crack in the SiN passivation ﬁlm. Notice that the crack opens substantially. Figure 26(d) is a cross-section of two aluminum pads, which shift and break the SiN ﬁlm. The main experimental observations are summarized as follows: * * * * * SX0445 Cracking occurs in the SiN ﬁlm at the die corners. The aluminum pads crawl toward the die center. The displacement reduces for pads away from the die corners. Cracking occurs after temperature cycles, and becomes more extensive as the number of cycles increases. Cracking occurs in the SiN ﬁlm over the metal ﬁlms, but not in the SiN ﬁlm over silica. Cracking is more likely when the metal ﬁlms are wide and the SiN ﬁlm is thin. SX0450 CSI : 08125 26 Reliability of Interconnect Structures Figure 25 (a) A photo of a ﬂip-chip package. (b) A schematic of cross-section of the package. (c) Magniﬁed view of the interconnect structure. SX0455 Because the organic substrate has a larger thermal expansion coefﬁcient than the silicon die, upon cooling from the curing temperature, a shear stress develops on the silicon die. The shear stress concentrates at the die corners, and decreases away from the corners. As illustrated in Figure 27, the entire range of cyclic temperature is below the epoxy curing temperature, so that the shear stress at the die corners point toward the die center during cycling. It is not surprising that failures occur at the die corners, and that aluminum pads crawl toward the die center. Two questions, however, are inexplicable from these simple considerations. Why should crawling and cracking occur at all? The shear stress on the die is transmitted through the polymers, and is limited by the yield strength of the polymers, say 100 MPa. The yield strength of the metal ﬁlm exceeds 100 MPa (bib95 Nix, 1989). The fracture strength of the SiN thin ﬁlm is on the order 1 GPa (bib85 Ma et al., 1998). Why should cracks occur after many SX0460 CSI : 08125 Ratcheting 27 Figure 26 (a) The plan view of the surface of a die, near a die corner (source bib57 Huang et al., 2000). (b) Patterned aluminum pads. Cracks form in SiN over aluminum, but not in SiN over silica (source bib56 Huang et al., 2002). (c) A cross-section shows a crack in SiN (courtesy of Dr. J. B. Han). (d) A cross-section shows shifted aluminum pads (source bib55 Huang et al., 2001). temperature cycles? Unlike ductile materials, SiN does not have an intrinsic fatigue mechanism. 8.7.4.2 SX0465 Ratcheting toward a Steady State bib57 Huang et al. (2000) have recently discovered a mechanism that answers these questions. As mentioned before, the silicon die and the packaging substrate have different thermal expansion coefﬁcients, inducing shear stresses, t0, at the die corners upon curing (Figure 28). When the temperature cycles in a range below the curing temperature, the direction of the shear stress t0 is biased toward the die center. For simplicity, t0 is taken to be constant, set by the yield strength of the polymer, independent of position and temperature. The shear stress t0 is partly sustained by a membrane stress s in the passivation ﬁlm, and Figure 27 Temperature as a function of time. The cyclic temperature range is below the curing temperature of epoxy. CSI : 08125 28 Reliability of Interconnect Structures partly transmitted to the metal ﬁlm underneath as a shear stress in the metal, tm. The metal ﬁlm also has a large thermal expansion mismatch with silicon and silica beneath, so that the metal ﬁlm plastically yields in every temperature cycle. Because the temperature change by itself causes the metal to yield, even a very small shear stress in the metal, tm, will cause the metal to deform in shear plastically. The inplane plastic strain in the metal ﬁlm is constrained by the elastic substrate. Consequently, the amount of plastic shear strain per cycle in the metal is small, as will become evident later when we look at the model closely. The increment of the shear strain is in the same direction as the shear stress on the passivation ﬁlm, t0, pointing toward the center of the die. Incrementally, the shear stress in the metal ﬁlm, tm, relaxes, and the membrane stress s in the overlaying SiN ﬁlm builds up. It is this evolving stress state that cracks the SiN ﬁlm after some cycles. Figure 29 illustrates the evolution of the stress ﬁeld as the temperature cycles. In the ﬁrst temperature cycle, the shear stress t0 from the organic substrate is transmitted into the metal ﬁlm underneath the SiN ﬁlm, so that the stress in the SiN ﬁlm is low, comparable to t0 (Figure 29(a)). As the temperature cycles, the shear stress in the metal pad decreases, and the stress in SiN accumulates. After many cycles, a steady state is reached, in which the metal no longer has any shear stress (Figure 29(b)). The shear stress t0 from the organic substrate is Figure 28 At a corner of the die, the organic substrate applies a shear stress on the surface of the die. The shear stress points to the die center. The thermal expansion misﬁt between aluminum and silicon causes the aluminum pad to yield repeatedly during temperature cycles. Directed by the biased shear stress, the aluminum pad shears by a small amount each temperature cycle. After many cycles, the accumulated shear signiﬁcantly distorts the SiN ﬁlm, leading to cracking. Figure 29 The evolving stress state in the SiN ﬁlm and the aluminum pad. (a) Before temperature cycling, the shear stress due to the organic substrate is transmitted to the aluminum pad, and the structure does not distort much. (b) After many temperature cycles, the shear stress in aluminum vanishes, and the structure distorts greatly. (c) The shear stress from the organic substrate is balanced by the membrane stress in SiN. SX0470 CSI : 08125 Ratcheting 29 now all sustained by the membrane stress in the SiN ﬁlm. Figure 29(c) shows the free-body diagram of the SiN ﬁlm. Denote by sA the magnitude of the membrane stress in SiN at the two ends, tensile on the left and compressive on the right. As discussed above, the ﬁlm has the traction t0 on the top face from the organic substrate, but no traction on the bottom face from the metal pad. Force balance requires that sA ¼ t0 L ; 2t ð68Þ where t is the thickness of the SiN ﬁlm and L the length of the aluminum pad. Although the shear stress t0 is small, the length ratio L/t is typically very large. Consequently, the stress in the SiN ﬁlm can build to a high level to cause cracking. The magnitude of the stress in the SiN ﬁlm increases with the shear stress at the die corner and the width of the aluminum pad, but is inversely proportional to the SiN ﬁlm thickness. These are consistent with the experimental observations. In the steady state, the membrane stress in SiN varies linearly with the position, given by sðxÞ ¼ 2sA x=L; SX0475 SX0480 SX0485 ð69Þ where x is the distance from the center of the aluminum pad. Finite element calculation of a plane-strain model has conﬁrmed the main features of the model (bib57 Huang et al., 2000). As the temperature cycles, the shear stress in the metal reduces, and the membrane stress in the SiN ﬁlm increases. In the steady state, the shear stress in the metal vanishes, the in-plane stress in the metal cycles with the temperature, and the membrane stress in the SiN ﬁlm attains the distribution (69). The deformation in the same direction, guided by a bias and facilitated by a cyclic load (temperature change in this case), is known as ratcheting deformation (bib17 Bree, 1967; bib63 Jansson and Leckie, 1992; bib115 Suresh, 1998). In addition to the example discussed here, several other examples of ratcheting deformation in thin ﬁlm structures have been discovered (bib43 He et al., 2000; bib10 Begley and Evans, 2001; bib65 Karlsson and Evans, 2001). To avert SiN cracking, an industrial practice is to change the shape and the size of the metal pad. For example, slots are made in the metal pads, so that the SiN ﬁlm is in contact with the silica in the slots (Figure 30). To aid design, we would like to do calculations over thousands of temperature cycles, for three-dimensional structures, and for many geometrical designs. Figure 30 (a) An aluminum pad on silica surface. (b) and (c) The aluminum pads are slotted. In each case, a SiN ﬁlm covers both aluminum and silica. However, because of the nonlinear material behavior, each temperature rise or drop has to be divided into many small steps in the ﬁnite element calculation. A crude division would lead to numerical ratcheting, i.e., the apparent ratcheting deformation due to accumulated numerical errors for structures that should not suffer ratcheting at all. Consequently, direct ﬁnite element calculation would require too much time to be practical. In the steady state, the shear stress in the metal pad vanishes, and the SiN ﬁlm is in a state of plane-stress elastic deformation. At the edges of the metal pad, the displacement of the SiN ﬁlm is constrained by the silica, and is set to be zero. The shear stress from the organic substrate is distributed over the face of the SiN ﬁlm, acting like a body force. Such a linear elastic plane-stress problem can be solved rapidly by the ﬁnite element method for any pad geometry. As an illustration, Figure 31(a) shows the normalized maximum principal stress distribution at the steady state by applying the uniform shear stress t0 in the direction of 451 from the x-axis. The membrane stresses in the passivation ﬁlm scale with t0L/hp, where L is the width of the metal ﬁlm. The maximum principal tensile stress is very high near the left edge and the left upper corner, where cracking always happens. Figure 31(b) shows a slotted structure, where the membrane stress in the passivation ﬁlm is greatly reduced. The steady state is a robust concept: it does not depend on the detailed mechanical property of the metal, and the stress ﬁeld is easy to calculate. The steady state is applicable even if the metal creeps, or the passivation ﬁlm and the metal debond. Once the stress ﬁeld in the steady state is calculated, one can ascertain if the SiN ﬁlm is safe from cracking. If SiN can SX0490 SX0495 CSI : 08125 30 Reliability of Interconnect Structures Figure 31 The normalized maximum principal stress distribution, (smax hp)/(t0L). The length L is taken to be the width of the metal ﬁlm. (a) A rectangular aluminum pad and (b) a slotted aluminum pad (source bib57 Huang et al., 2002). SX0500 sustain the stress in the steady state, then the design is immortal: it can sustain any number of temperature cycles without cracking. This steady state approach leaves two issues unresolved: the condition under which the metal ﬁlm undergoes ratcheting deformation, and the number of cycles needed to approach the steady state. We study these issues in the following sections. To gain insight, we examine idealized structures and material behaviors. 8.7.4.3 SX0505 Shakedown vs Cyclic Plastic Deformation First consider a blanket metal ﬁlm bonded to a substrate. The ﬁlm has thermal expansion coefﬁcient am, Young’s modulus Em, and Poisson’s ratio nm. We model the ﬁlm as a nonhardening solid, assuming that the yield strength Y is independent of temperature, and is the same under tension and compression. Subject to a temperature change, the ﬁlm is under biaxial stress s. The substrate, being much thicker than the ﬁlm, has negligible stress, so that only its thermal expansion coefﬁcient as enters the consideration. The ﬁlm and the substrate are well bonded, matching the net strain at all time. When the temperature changes by dT, the ﬁlm and the substrate acquire thermal strains amdT and asdT, respectively. This mismatch is compensated in different ways, depending on whether the ﬁlm is elastic or plastic. If the ﬁlm is elastic, |s|oY, the mismatch in the thermal strains is compensated by the change in the elastic strain in the ﬁlm. The latter gives rise to the change in the ﬁlm stress: ds ¼ Em ðam as Þ dT: 1 nm ð70Þ If the ﬁlm yields, however, the stress in the ﬁlm is ﬁxed at the yield strength, either in tension s ¼ þ Y or in compression s ¼ Y, so that the elastic strain in the ﬁlm no longer changes with the temperature. Consequently, the mismatch in the thermal strains is compensated by the SX0510 CSI : 08125 Ratcheting plastic strain in the ﬁlm: p de ¼ ðam as Þ dT: SX0515 ð71Þ Figure 32 plots the change in the ﬁlm stress s and the plastic strain ep when the temperature cycles between TL and TH. Let us start at the preset high temperature TH, with the initial ﬁlm stress s0 anywhere between Y and þ Y. (1) As the temperature drops, the ﬁlm is elastic, and the ﬁlm stress changes toward tension according to Equation (70). The plastic strain does not change. (2) At some temperature TA, the ﬁlm yields in tension, and the ﬁlm stress is ﬁxed at the yield strength, s ¼ þ Y. As the temperature drops, the plastic strain increases according to (71). (3) On reaching the preset low temperature TL, the temperature starts to rise. The ﬁlm is elastic, and the ﬁlm stress changes toward compression. The plastic strain does not change. (4) At some temperature TB, the ﬁlm yields in compression, and the ﬁlm stress is ﬁxed at the yield strength, s ¼ Y. The plastic strain decreases as the temperature rises. (5) On reaching TH, the temperature starts to drop again. The ﬁlm is elastic, and the ﬁlm stress changes toward tension. The plastic strain does not change. Afterwards, the stress and strain state of the ﬁlm cycles with the temperature. Inspecting Figure 32, we distinguish three behaviors. Imagine that TL is ﬁxed, and TH is allowed to change. If TL4TA, the ﬁlm will be elastic during temperature cycling. If THoTB, the ﬁlm will undergo plastic deformation in the ﬁrst cycle, but will be elastic in all subsequent cycles. This behavior is referred to as shakedown. The ﬁlm reaches the shakedown condition if Em ðam as ÞðTH TL Þ o2: ð1 nm ÞY SX0520 ð72Þ If the inequality (72) is reversed, the ﬁlm will undergo cyclic plastic deformation. During the fabrication of the interconnect structure, the metal ﬁlm inevitably yields as the temperature drops from the processing temperature. Consequently, plastic yield during the ﬁrst cycle should not be of any concern, and the elastic and shakedown behaviors are practically indistinguishable. However, as we will see below, the difference between shakedown and cyclic plasticity has a signiﬁcant consequence. The demarcation (72) between the two regimes, shakedown and cyclic plasticity, is unaffected by the initial ﬁlm stress. 8.7.4.4 Figure 32 Plastic strain and stress change with the temperature during a thermal cycle of blanket aluminum ﬁlm on a silicon substrate. 31 Ratcheting Strain Rate In the above, the plastic strain cycles because the ﬁlm has to match the net in-plane strain to the substrate. By contrast, the shear strain in the ﬁlm is not constrained by the substrate, so that it may accumulate under certain conditions. bib55 Huang et al. (2001) have calculated the strain rate due to ratcheting. Figure 33(a) illustrates a blanket metal ﬁlm bonded on a semi-inﬁnite elastic substrate. A shear stress tm acts on the surface of the metal ﬁlm. For the time being, this shear stress is taken to be spatially uniform, and remains constant as the temperature cycles. The stress ﬁeld in the structure is very simple. The semi-inﬁnite substrate is subject to the same shear stress tm, but no other stress components. Let the coordinates in the plane of the ﬁlm be x1 and x2, the coordinate normal to the plane be x3, and the coordinate x1 coincide with the direction of the shear stress tm. As shown in Figure 33(b), the ﬁlm is in a uniform stress SX0525 CSI : 08125 32 Reliability of Interconnect Structures state of a combination of a biaxial stress and a shear stress: s11 ¼ s22 ¼ sm ; SX0530 s13 ¼ tm ; s23 ¼ s12 ¼ 0: ð73Þ The biaxial stress sm changes with the temperature. Obviously, the uniform stress states in the substrate and in the ﬁlm satisfy the equilibrium conditions. To model plastic deformation in the metal ﬁlm, we adopt the J2 ﬂow theory (bib44 Hill, 1950). The deviatoric stress tensor, sij ¼ sij skk dij =3; has the components s11 ¼ s22 ¼ sm =3; s23 ¼ s12 ¼ 0: s33 ¼ 2sm =3; s13 ¼ tm ; ð74Þ The Mises yield condition, 3sij sij =2 ¼ Y 2 ; is specialized to s2m þ 3t2m ¼ Y 2 : ð75Þ The yield condition is an ellipse on the sm–tm plane (Figure 33(c)). The metal ﬁlm is elastic when the stress state is inside the ellipse, and yields when the stress state is on the ellipse. The stress state outside the ellipse is unreachable. When the ﬁlm yields, for a given tm, the biaxial stress can only be at one of the two levels: sm ¼ 7 qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Y 2 3t2m : ð76Þ These two states, tensile and compressive, are indicated in Figure 33(c). Figure 33 (a) A blanket aluminum ﬁlm on a silicon substrate. (b) The stress state in the aluminum ﬁlm consists of biaxial in-plane stresses and a shear stress. (c) The yield condition on the sm–tm plane. CSI : 08125 Ratcheting SX0535 Figure 34 shows a coordinate plane spanned by the normalized shear stress, tm/Y, and the normalized temperature range, Eðaf as ÞðTH TL Þ=½ð1 nÞY : The plane is divided into three regimes: plastic collapse, shakedown, pﬃﬃﬃ and crawling. If tm =Y Z1= 3; the ﬁlm plastically deforms under the shear stress alone without the aid of the temperature change, and is in the pﬃﬃﬃ plastic collapse regime. If tm =Y o1= 3 and the temperature range is small enough, the ﬁlm may plastically deform during the ﬁrst temperature cycle, but cycles elastically afterwards. The ﬁlm is in the shakedown regime. This shakedown condition is represented in Figure 34 by a shaded region below a quarter of an ellipse: rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ t 2ﬃ Eðaf as ÞðTH TL Þ m ¼2 13 : ð77Þ ð1 nÞY Y 33 the plastic strain tensor points in the direction normal to the yield surface (Figure 33(c)). During plastic deformation, dep has the same sign as the biaxial stress sm, and dgp has the same sign as the shear stress tm. When ﬁlm yields in compression (smo0), the plastic inplane strain decreases, depo0. When ﬁlm yields in tension (sm40), the plastic in-plane strain increases, dep40. Because the ﬁlm is bonded to the substrate, for a given temperature increment, dep is always ﬁnite. Consequently, in each cycle, gp increases by a ﬁnite amount in the direction of tm, both when the ﬁlm is in tension and in compression. When the ﬁlm yields, the plastic in-plane strain changes according to Equation (71). A substitution into (78) gives the increment of the plastic shear strain: dgp ¼ SX0536 The J2 ﬂow theory dictates that the plastic strain increment tensor be in the same direction as the deviatoric stress tensor, namely, deij ¼ spij dl; where dl is a scalar. Consequently, from Equation (74) we obtain that dep dgp ¼ ; sm =3 2tm ð78Þ where gp ¼ 2ep13 is the plastic shear strain in the ﬁlm. Equation (78) is the key to the understanding of metal ﬁlm crawling. Its geometric interpretation is well known: the increment of 6tm ðam as Þ dT: sm SX0545 ð79Þ When the ﬁlm plastically deforms in tension, pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ sm ¼ þ Y 2 3t2m and dTo0. When the ﬁlm plastically deforms in compression, sm ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ Y 2 3t2m and dT40. In either case, the plastic shear strain increment is in the direction of tm, namely, dgp40, giving rise to crawling. In Figure 34, above the shakedown regime, if tm ¼ 0, the temperature change causes cyclic inplane strain but no shear strain. However, this cyclic state is unstable. Any shear stress tm, however small, will cause the ﬁlm to crawl. In the crawling regime, the in-plane strain cycles Figure 34 Various regimes on the plane spanned by the normalized shear stress in metal and the normalized temperature range. SX0550 CSI : 08125 34 Reliability of Interconnect Structures Figure 35 Shear stress as a function of the ratcheting strain rate. plastically, but the shear strain increases by a ﬁxed amount each cycle, given by ison between Equations (80) and (81) gives " # 12ð1 nm Þtm Em ðam as ÞðTH TL Þ p pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 : Dg ¼ Em ð1 nm Þ Y 2 3t2m ZR ¼ ð80Þ SX0555 SX0560 Figure 35 plots the ratcheting strain per cycle, Dgp, as a function of the shear stress, tm. We make an analogy between the strain per temperature cycle (i.e., the ratcheting rate) and the strain per unit time (i.e., the strain rate). Figure 35 is thus analogous to the relation between strain rate and stress in viscous ﬂow. In general, we write the ratcheting rate law as qgp/qN ¼ f(tm). The shear pﬃﬃﬃ stress should be bounded as tm =Y o1= 3; otherwise, the ﬁlm has unlimited plastic shear strain even without pﬃﬃﬃ the temperature change. As tm =Y -1= 3; the ratcheting rate becomes large for any given temperature ranges. Depending on the temperature range, we distinguish several behaviors as follows. When Em(amas) (THTL)/[(1nm)Y]>2, the temperature change by itself can cause the metal ﬁlm to deform plastically in every cycle. When the shear stress is zero, the metal ﬁlm undergoes cyclic in-plane plastic deformation, and has no shear strain. When the shear stress is small, the ratcheting rate is linearly proportional to the shear stress: qgp tm ¼ : qN ZR ð81Þ We call ZR the ratcheting viscosity. A compar- 1 Em Eðam as ÞðTH TL Þ 2 : ð82Þ ð1 nm ÞY 12ð1 nm Þ The linear ratcheting is analogous to the Newtonian viscous ﬂow. The ratcheting viscosity has the dimension of elastic modulus, and increases when the temperature range decreases. We will mainly use the linear ratcheting approximation (82) in the subsequent development. When Em(amas) (THTL)/[(1nm)Y]o2, the metal ﬁlm yields only when the shear stress exceeds a critical value, namely, when the quantity in the bracket in Equation (80) is positive. As seen in Figure 35, this behavior is analogous to the Bingham viscous ﬂow. When Em(amas) (THTL)/[(1nm)Y] ¼ 2, for small shear stress, Equation (80) gives rise to a power-law behavior, qgp =qNBt3m : 8.7.4.5 SX0565 SX0570 The Transient Process to Approach the Steady State bib56 Huang et al. (2002) have developed a one-dimensional model of ratcheting of the thin ﬁlm structures. As shown in Figure 36, a metal ﬁlm is in a thick elastic substrate, and the passivation thin ﬁlm is on the metal ﬁlm and the substrate. A constant shear stress, t0, due to the packaging substrate, is applied on the passivation ﬁlm. The metal ﬁlm is of thickness H and length L. The passivation ﬁlm is of thickness h. Cycle the structure between TH and TL. The shear stress in the metal ﬁlm is tm, and the normal stress in the passivation ﬁlm is SX0575 CSI : 08125 Ratcheting 35 Figure 36 Illustration of one-dimensional structure of passivation ﬁlm on the metal ﬁlm and substrate. The insets show the different elements and the stress states of the passivation ﬁlm, and the stress and ﬂow in the metal ﬁlm. SX0580 s. Now both tm and s are allowed to vary with the number of cycles, N, and the position, x. We expect tm to vary slowly with N and x, so that we will use the ratcheting rate law obtained in the last section. First look at the elastic passivation ﬁlm. As shown in the inset in Figure 36, the passivation ﬁlm is subjected to a membrane stress s(N, x), a constant shear stress t0 on the top surface, and a variable shear stress tm(N, x) on the bottom surface. The force balance of the differential element requires that qs tm t0 ¼ : qx h ð83Þ Let u(N, x) be the displacement of the passivation ﬁlm in the x-direction. Elasticity of the passivation ﬁlm requires that s ¼ Ep SX0585 qu : HqN ð86Þ We introduce the ratcheting diffusivity as DR ¼ Ep hH=ZR : ð87Þ Equation (86) is a diffusion equation with a source term. We assume no separation between the metal ﬁlm and the substrate, so that the displacement of the metal ﬁlm at the two edges is the same as the displacement of the substrate. As the substrate is semi-inﬁnite and elastic, its displacement is negligible compared to the accumulated displacement in the passivation ﬁlm. Consequently, the boundary conditions for the displacement of the passivation ﬁlm are u¼0 at x ¼ 7L=2 for all N: SX0595 ð88Þ ð84Þ where Ep is Young’s modulus of the passivation ﬁlm. Next look at the ratcheting metal ﬁlm. The shear strain relates to the displacement as gp ¼ u=H: We assume that the temperature range is large, Em(amas) (THTL)/[(1nm)Y]>2. Consequently, we adopt the shear stress and plastic shear strain increment relation (13) as tm ¼ ZR SX0590 qu ; qx qu q2 u Ht0 : ¼ DR 2 þ ZR qN qx ð85Þ The ratcheting viscosity ZR is deﬁned by Equation (82). Substituting Equations (84) and (85) into Equation (83) gives the governing equation: Because the temperature range is large enough to cause the metal to yield in every cycle, so long as there exists a shear stress tm in the metal, the metal will ratchet. After many temperature cycles, the structure will reach the steady state, in which the shear stress in the metal ﬁlm vanishes, tm ¼ 0, but the cycling temperature still causes the metal ﬁlm to yield cyclically. The steady state can be obtained by setting qu/qN ¼ 0 and satisfying the boundary conditions (88). In the steady state, t0 is fully sustained by the membrane stress in the passivation ﬁlm, giving rise to a linear membrane stress distribution (69). Analogous to any diffusion problem, the characteristic number of cycles to reach the SX0600 SX0605 CSI : 08125 36 Reliability of Interconnect Structures steady state can be estimated by NC ¼ L2/DR, or NC ¼ SX0610 ð89Þ The number NC can be large mainly because the ratio L2/(hH) is large. If one replaces the metal ﬁlm with a plastically deformable polymer, the ratio of elastic modulus of the polymer and the passivation is small, which would signiﬁcantly reduce NC. Note that NC is independent of t0. In the above, the metal ﬁlm is taken to be a nonhardening material in this model. This corresponds to a safe engineering design, as the hardening metal ﬁlm can reduce the ratcheting effects (bib55 Huang et al., 2001). The model can also be easily extended to consider the nonlinearity of the ratcheting viscosity by using the ﬁnite difference method. The stress concentration at the edges needs to be treated better, as the maximum tensile stress in the passivation ﬁlm is at the corner. Fracture conditions also need to be considered more carefully. Several useful rules for design are evident. First, one should aim to avoid metal ﬁlm ratcheting altogether. Under cyclic temperature, the metal ﬁlm cycles elastically if the temperature range is small and the yield strength of the metal is large, according to (77). Second, if one cannot avoid ratcheting, one may aim to design the metal ﬁlm geometry such that the passivation ﬁlm can sustain the steady state, in which the stress distribution in the passivation ﬁlm can be calculated by solving a linear elastic plane-stress problem. Third, if the characteristic number NC is much larger than the number of cycles required by the qualiﬁcation test, one may design according to the transient stress state, solving the stress ﬁeld as a function of the number of cycles. The present model allows one to evaluate these options in design. 8.7.4.6 SX0615 L2 Em hH 12Ep ð1 nm Þ 1 Em ðam af ÞðTH TL Þ 2 : ð1 nm ÞY Ratcheting-induced Crack Growth Consider the structure illustrated in Figure 10 again. In the present context, a brittle ﬁlm lies on a metal underlayer, which in turn lies on a rigid substrate. Cycle the structure between temperatures TL and TH. Within the temperature and time of the experiment, the metal does not creep, but can have time-independent plastic deformation. For simplicity, assume that the tensile stress in the uncracked blanket ﬁlm, s, is constant as the temperature changes. This happens in practice when the elastic ﬁlm and the substrate have a similar coefﬁcient of thermal expansion, and s is due to the deposition process or an applied load. As temperature cycles, the metal layer undergoes ratcheting plastic deformation. The stress ﬁeld in the ﬁlm relaxes in the crack wake, and intensiﬁes around the crack tip. By the ratcheting-creep analogy, we rewrite the scaling law for the crack velocity (38) as the scaling law for crack growth per cycle (bib78 Liang et al., 2002a): da Hhs2 ¼ 0:6 ; dN ZR G ð90Þ where ZR is given by (82), and G is the fracture energy of the brittle ﬁlm. 8.7.5 STRESS-INDUCED VOIDING This section begins with a description of stress-induced voiding (SIV), followed by an analysis of its main features: saturated void volume, resistance change, stress generation, void initiation, void growth, and stress relaxation. We then give an analytical model of nonhydrostatic stress state in an elastic–plastic interconnect line encapsulated in a dielectric. An observation of SIV in blanket copper ﬁlms is discussed. We ﬁnally consider the effects of low-k dielectrics and barriers. bib98 Okabayashi (1993) and bib114 Sullivan (1996) have provided two reviews on SIV. This section will focus on physical descriptions of the phenomenon, leaving the design implications to the next section, after we have studied electromigration. 8.7.5.1 SX0620 Stress-Induced Voiding in Encapsulated Metal Line Early aluminum lines had the width much larger than the thickness. They behaved like blanket ﬁlms. When narrow aluminum lines were introduced, voids were observed on wafers held in ovens, or even on wafers left on shelves at room temperature (bib24 Curry et al., 1984; bib140 Yue et al., 1985; bib128 Turner and Wendel, 1985). The voids may be crack-like or rounded, grow with time, and sever the interconnects (Figure 37). A basic understanding soon followed (bib64 Jones and Basehore, 1987; bib45 Hinode et al., 1990; bib38 Greenebaum et al., 1991; bib68 Korhonen et al., 1991; bib106 Sauter and Nix, 1992). Aluminum has a larger thermal expansion coefﬁcient than silica. Encapsulated in silica at a high temperature, on cooling, a narrow aluminum line is in a tensile, triaxial SX0625 SX0630 CSI : 08125 Stress-Induced Voiding 37 Figure 38 An encapsulated aluminum line is under triaxial tension. The stress vanishes at a ﬂaw. The stress gradient motivates aluminum atoms to diffuse in the line, and simultaneously grow the void and relax the stress. Figure 37 Voids grow in aluminum lines encapsulated in silica after some storage time. (a) Crack-like void and (b) rounded void. SX0635 stress state. The magnitude of the stress in aluminum readily exceeds the yield strength of aluminum. Indeed, even a liquid with zero yield strength, so encapsulated, would be under hydrostatic tension. Over a long time, a small piece of a crystal is like a liquid in that they both creep under shear. An encapsulated metal line under uniform hydrostatic tension is in a state of equilibrium: atoms have no motivation to diffuse from one place to another. However, this equilibrium state is metastable. A ﬂaw may act like a void nucleus. If the stress near the ﬂaw is low or vanishes, the nonuniform stress ﬁeld motivates aluminum atoms to diffuse away from the ﬂaw, simultaneously growing the void and relaxing the tensile stress (Figure 38). The metal line approaches a stable equilibrium state consisting of voids and unstressed metal. An accelerated testing method has also been developed, known as the high-temperature storage (HTS) test. The aluminum line is stress-free at a temperature T0, which is close to the silica deposition temperature. Samples are kept in an oven at some temperature T below T0. The thermal expansion mismatch volume scales with the temperature drop, Figure 39 As the temperature drops from the stress-free temperature T0, the misﬁt strain increases, but the atomic diffusivity decreases. For a given time duration, the void size maximizes at an intermediate temperature Tmax. T0T. It is this mismatch volume that feeds to the void. The atomic diffusivity depends on the temperature as D ¼ D0 exp (Q/kT), where k is Boltzmann’s constant, Q the activation energy, and D0 the frequency factor. As the temperature drops, the mismatch volume increases, but the diffusivity decreases (Figure 39). Consequently, voids grow fastest at a particular temperature Tmax. During the storage test, the electrical resistance of a line is measured as a function of time. The line fails if its resistance increases by, say 20%. The time to fail half of the lines, i.e., the median-time-tofailure (MTF), is ﬁt to a semi-empirical relation (bib90 McPherson and Dunn, 1987): MTF ¼ C ðT0 TÞN exp Q ; kT ð91Þ where C and N are ﬁtting parameters, along with T0 and Q. This relation captures the above physical considerations. The failure time approaches inﬁnity when the test is carried either CSI : 08125 38 SX0640 SX0645 AU:5 at the stress-free temperature T0, or at absolute zero. To obtain the ﬁtting parameters, the storage tests are carried out at several temperatures, possibly around Tmax to shorten the testing time. Equation (91) is then extrapolated to predict the failure time at, say, room temperature. SIV is mitigated in aluminum interconnects in several ways. First, adding a few percent of copper into aluminum reduces the diffusion rate by nearly two orders of magnitude (bib5 Ames et al., 1970). Second, materials of negligible diffusion rates, such as W and TiN, are used as shunts (Figure 38), so that a void in the aluminum line does not open the circuit, but just increases the electrical resistance somewhat (bib48 Howard et al., 1978). Third, a short aluminum line cannot grow a large void, because the volume of material to be relaxed is small (bib32 Filippi et al., 1995). These measures were all originally developed to mitigate electromigration voiding. The interest in SIV resurged during the later 1990s since copper lines entered the interconnect structure. Voids have been observed in electron beam evaporated copper lines, and found to be sensitive to the texture (bib66 Keller et al., 1997). On-chip copper lines are electroplated, and have small initial grains. If the lines are not properly annealed before encapsulation, later annealing will cause grain growth, densify copper, and induce voids (bib47 Hommel et al., 2001; bib96 Ogawa et al., 2002). In aluminum interconnects, voids grow in the lines, but not in the tungsten vias. By contrast, in copper interconnects, vias themselves are made of copper, and are susceptible to voiding (Figure 40). Furthermore, compared to aluminum, copper has large yield strength and a high degree of elastic anisotropy. Stress concentration arises at the junction of the copper grain boundary and SiN top layer; voids have been observed even in blanket copper ﬁlms (bib109 Shaw et al., 2001; bib107 Sekiguchi, 2001). 8.7.5.2 SX0650 Reliability of Interconnect Structures An Analysis of Stress-Induced Voiding Despite efforts in for nearly two decades (1980s and 1990s), there is no single model that accounts for all aspects of SIV. Complicated factors (e.g., grain structures, ﬂaws, interfaces, and atomic transport mechanisms) play roles. Detailed information of such factors is incompletely known, and will probably never be precisely controlled in fabrication. At this point, it seems desirable to consider the physics of the phenomenon semi-quantitatively. In this Figure 40 In the copper interconnect structure, vias are also made of copper, and are susceptible to stress-induced voiding. spirit, the following sub-models are given in outline. (i) Saturated Void Volume (SVV) An encapsulated metal line is stress free at a high temperature T0, and is cooled to the storage test temperature T. The total number of atoms in the line is constant at all time. Because atomic transport does not change the volume of the metal, the thermal misﬁt strain is accommodated by a combination of void space and elastic deformation. When the stress in the line completely relaxes, the thermal expansion misﬁt is fully accommodated by the void space. The saturated void volume (SVV) is Vsn ¼ 3DaðT0 TÞ V ; ð92Þ where V is the volume of the metal line, and Da is the effective thermal expansion mismatch strain. If a metal line were embedded in silicon, Da ¼ amaSi, where am and aSi are the thermal expansion coefﬁcients of the metal and silicon, respectively (am ¼ 24 106 K1 for aluminum and 17 106 K1 for copper). In an interconnect structure, however, Da depends on all materials in the structure. For the silica-based interconnect structure, because the metals have much larger thermal expansion coefﬁcients than the surrounding materials (silica, silicon, silicon nitride, and tantalum), the thermal expansion mismatch is insensitive to which exact value is used for these other materials; we SX0655 CSI : 08125 Stress-Induced Voiding SX0660 SX0665 SX0670 39 will use Da ¼ am4 106 K1 in the following estimates. A representative stress-free temperature is 4001C, and a representative storage test temperature is 2001C. Taking these values, one ﬁnds that Vsn/V ¼ 1.2% for aluminum, and Vsn/V ¼ 0.78% for copper. For a line of size 1 mm 1 mm 10 mm, the saturated void, if it is a single spherical one, has radius 306 nm for aluminum, and 265 nm for copper. The interconnect structure with low-k dielectrics will be discussed in Section 8.7.5.6. Many voids may nucleate along the metal line, each growing to relax stress in its vicinity. Once the stress completely relaxes, the sum of the volumes of all the voids remains constant as the line is held at the constant temperature. Equation (92) gives this sum. The actual void volume can be larger or smaller than the SVV. When a line is cooled to a low temperature for a short time, the tensile stress partially relaxes, so that the total void volume is smaller than the SVV. If the line is then brought to a high temperature, for some time the metal is under compression, and the void volume is larger than the SVV. In case of a copper line, we assume that the electroplated copper has been annealed to allow densiﬁcation prior to encapsulation, so that only thermal expansion mismatch contributes to void volume. Figure 41 (a) Void length smaller than tungsten stud diameter and (b) void length larger than tungsten stud diameter. (ii) Resistance Increase increase is A line fails when the voids signiﬁcantly increase the resistance of the line. The resistance change does not uniquely relate to the void volume. Small, isolated voids do not cause as much resistance increase as a single large void that depletes a segment of the metal line. Even when only one void is left near a via, the resistance change depends on geometry. Figure 41 compares two identical voids, the only difference being the size of the tungsten studs relative to the void. Evidently, the resistance increases in Figure 41(a) is smaller than that in Figure 41(b). When the void length exceeds several times the linewidth, the resistance increase can be estimated from the void length. Let r be the resistivity of the interconnect, L its length, and A its cross-sectional area. The resistance of a void-free interconnect is R ¼ rL/A, ignoring the conductance due to the aluminide shunt layers. Let r1 and A1 be the resistivity and the cross-sectional area of the aluminide layers. When a void of length L1 appears in the line, current ﬂows in the aluminide layers, and the resistance increases by DR ¼ r1L1/A1, where the resistance of aluminum of length L1 is neglected. Consequently, the relative resistance DR r1 L1 =A1 ¼ : R rL=A ð93Þ Everything else being equal, the thicker the shunt layers, the smaller the resistance change. Taking r1/r ¼ 10, A1/A ¼ 0.1, and L1/ L ¼ 1.0%, one ﬁnds that DR/R ¼ 100%. (iii) Hydrostatic Tension in Encapsulated Metal Line The stress ﬁeld in the metal line is complicated in general, with tensor components and nonuniformity along the line. To grow a large void, atoms must diffuse in the line over a length much larger than the linewidth. On such a timescale, creep should have relaxed each point in the line to a hydrostatic state (bib68 Korhonen et al., 1991). That is, over a sufﬁcient long timescale, at an elevated temperature, a crystal behaves like a liquid. The hydrostatic stress in the metal line prior to voiding can be calculated as follows. Figure 42 illustrates separately the metal line and the dielectric. In the metal line, the stress state has components of an equal magnitude s in all directions. The stress causes the metal to SX0675 CSI : 08125 40 Reliability of Interconnect Structures This equation deﬁnes an effective modulus meff. This effective modulus depends on the shape of the hole, as well as the elastic constants of the dielectric, the barrier, and the silicon substrate. The effective modulus can be readily calculated using the ﬁnite element method (Section 8.7.5.6). If the cross-section is a long rectangle, rather than a square, the system is more compliant, leading to a small meff. In the idealized case, when the hole has a circular cross-section, and the dielectric is inﬁnite, the stress ﬁeld in the dielectric is known analytically, and we ﬁnd that the effective modulus is meff ¼ Ed/2(1 þ nd), coincident with the shear modulus of the dielectric. Let y be the volumetric strain caused, e.g., by the mismatch in thermal expansion coefﬁcients, or densiﬁcation, or atomic diffusion. This volumetric strain is accommodated by the difference in the volume change of the interconnect line and that of the dielectric hole. Combining the two contributions, one relates the hydrostatic stress in the metal, s, to the volumetric mismatch strain between the metal and the encapsulation, y, namely, s ¼ By; ð95Þ with the effective modulus B given by Figure 42 Consider separately the metal line as a cylinder and the dielectric as a solid with a hole. SX0680 expand with the volumetric elastic strain s/Bm, where Bm is the bulk modulus of the metal. When the metal is modeled as an isotropic material, the bulk modulus relates to Young’s modulus Em and Poisson’s ratio nm as Bm ¼ Em/3(12nm). For a metal of cubic crystalline symmetry, the bulk modulus relates to its crystalline elastic constants as Bm ¼ (C11 þ 2C12)/3. For aluminum, C11 ¼ 108 GPa; C12 ¼ 62 GPa; C44 ¼ 28 GPa; giving Bm ¼ 77 GPa. For Copper, C11 ¼ 168 GPa; C12 ¼ 121 GPa; C44 ¼ 75 GPa; giving Bm ¼ 136 GPa. Regard the encapsulation as an elastic solid with a hole subject to a normal traction of magnitude s. The dielectric is in a state of plane-strain deformation. The traction causes Rthe cross-sectional area of the hole to reduce by un ds; where un is the normal component of the elastic displacement at the hole surface. Let A be the cross-sectional area of the hole. Linearity of the elastic ﬁeld requires that 1 A Z un ds ¼ s : meff ð94Þ 1 1 1 þ : ¼ B Bm meff ð96Þ If the cross-section is a long rectangle, the effective modus is small, leading to a low hydrostatic stress. In the limiting case when the interconnect is a blanket ﬁlm, the hydrostatic stress vanishes in this liquid-like model. For an interconnect of a square cross-section, taking meff ¼ 30 GPa for silica, the effective modulus is B ¼ 22 GPa for aluminum/silica structure, and B ¼ 24 GPa for copper/silica structure. The mismatch strain is mainly accommodated by the elastic deformation of the dielectric, so that the effective moduli of the two structures are similar, despite the nearly factor 2 difference in the bulk moduli of aluminum and copper. The effective modulus reduces if the cross-section is a long rectangle. Assume that the volumetric strain is entirely due to the thermal expansion mismatch between the metal and the dielectric, y ¼ 3Da(T0T). For the temperature drop T0 T ¼ 200 K, the hydrostatic stress is s ¼ 260 MPa in aluminum line, and s ¼ 187 MPa in copper line. Some authors have treated the dielectric as a rigid material, and taken the bulk modulus of the metal, Bm, as the effective modulus. This would signiﬁcantly overestimate the effective modulus (Bm/ B ¼ 3.5 for aluminum and Bm/B ¼ 5.7 for copper). SX0685 CSI : 08125 Stress-Induced Voiding (iv) Void Initiation SX0690 svoid ¼ 2g=a: Next consider a void-like ﬂaw in a metal subject to a hydrostatic stress. The void can change its size by relocating atoms from the void surface into the metal far away from the void. In doing so, the void increases its surface area, and the remote stress does work. The former increases the free energy, but the latter decreases it. Will the void shrink or enlarge? For the time being, we assume that the void volume changes slightly, so that the number of atoms transported into the line is so small that the stress s does not change. Take the solid without the void but under the same applied stress as the ground state, at which the system has zero free energy. The current state has a void of radius a. Let g be the surface energy per unit area. In creating the void, a surface of area 4pa2 is exposed, raising the free energy of the system by g4pa2. At the same time, atoms occupying the volume 4pa3/3 relocate, allowing the remote stress to do work s(4pa3/3). Thus, the free energy of the system, relative to that of solid with no void, is FðaÞ ¼ 4pa2 g 43 pa3 s: 41 ð97Þ Figure 43 sketches the free energy as a function of the void radius. When a ¼ 0, F ¼ 0, which is the ground state. When the void is small, the surface energy dominates, and the void shrinks to reduce the free energy. When the void is large, the stress dominates, and the void enlarges to reduce the free energy. The two behaviors are separated at a critical void radius a*, at which the free energy maximizes. The critical void radius is given by a* ¼ 2g/s. Taking representative values, g ¼ 1 J m2 and s ¼ 200 MPa, we ﬁnd that the critical radius is a* ¼ 10 nm. If the pre-existing ﬂaw size a is known, the ﬂaw can grow if the stress exceeds the value ð98Þ The use of this condition will be critiqued in Section 8.7.6.3. (v) Void Growth and Stress Relaxation Because the volumetric strain due to thermal expansion mismatch is on the order of 102, for a void to grow to a size to sever the line, a long length of the metal has to be relaxed. The long-range diffusion samples the averages of various quantities, and is a much more robust process than void initiation. bib69 Korhonen et al. (1993) formulated a model to study atomic diffusion in an encapsulated metal line. To study mass transport over a length exceeding several times the linewidth, one can assume that the stress state is hydrostatic, varying along the line and with time. Let the x-axis coincide with the line. The stress in the line is a function of position and time, s(x, t). The nonuniformity of the stress motivates atoms to diffuse to the region of large tension. When an atom is removed from a stress-free solid, and then added to another solid under hydrostatic tension s, the free energy reduces by Os, where O is the volume per atom in the metal. Consequently, the driving force to relocate atoms in the metal line is f ¼O qs : qx ð99Þ Let J be the atomic ﬂux, i.e., the number of atoms crossing per unit area per unit time. Write the Einstein relation as J¼ Df : OkT ð100Þ The diffusivity D is taken to be the average along the aluminum line. The ﬂux divergence gives rise to the volumetric strain per unit time, qy/qt ¼ OqJ/qx. Recall that the mismatch volumetric strain relates to the stress by s ¼ By. . Consequently, the stress rate is proportional to the ﬂux divergence: qs qJ ¼ BO : qt qx ð101Þ A combination of the above equations gives qs DBO q2 s : ¼ qt kT qx2 Figure 43 radius. The free energy as a function of void SX0695 ð102Þ This partial differential equation, together with suitable initial and boundary conditions, governs the evolving pressure distribution, s(x, t). SX0700 CSI : 08125 42 SX0705 Reliability of Interconnect Structures Solutions of practical interest can be found in (bib69 Korhonen et al., 1993). With reference to Figure 38, assume that the ﬂaw is already large enough so that the stress near the ﬂaw is zero. Equation (102) is identical to the usual diffusion equation, with the diffusivity-like quantity DBO/kT. The solution to this initial-boundary value problem is well known. The time for a void to relax a segment of interconnect of length l scales as l 2 kT : tl B DBO ð103Þ The void fails a line by increasing the resistance of the line to a designated value. Assume that void of length L1 corresponds to the failure. To grow a void of length L1, the segment of the metal line needed to be relaxed is about l ¼ L1/ 3(amad)(T0T). Inserting into (103), we obtain the lifetime 1 Q : tlife p exp kT B½ðam ad ÞðT0 TÞ2 ð104Þ This expression looks similar to (91). As noted before, the effective modulus B depends on the cross-section shape and the dielectric type. Other things being the same, a structure with a smaller B will lead to a longer lifetime. 8.7.5.3 SX0710 SX0715 Nonhydrostatic Stress State in Encapsulated Metal Line The presence of the yield strength causes a nonhydrostatic stress state in the metal line, and also increases the magnitude of all stress components. According to (98), a higher stress can activate a smaller ﬂaw to grow into a void. The stresses in encapsulated elastic plastic metal lines have been studied by using ﬁnite element methods (bib64 Jones and Basehore, 1987; bib38 Greenebaum et al., 1991; bib37 Gouldstone et al., 1998). To gain insight into this phenomenon, we give an analytical solution for an idealized model, in which a long metal line of cylindrical cross-section, radius a, is encapsulated in an inﬁnite dielectric (Figure 44). The dielectric is elastic, with Young’s modulus Ed, Poisson’s ratio nd, and thermal expansion coefﬁcient ad. The corresponding properties for the metal are Em, nm, and am. Now consider the metal and the dielectric separately as a cylinder and an inﬁnite solid with a cylindrical hole. The metal is under a uniform, triaxial stress ﬁeld, with a longitudinal component sL and two transverse components of equal magnitude sT. The transverse stress sT also acts on the hole surface in the dielectric. The dielectric is taken Figure 44 The metal is under a triaxial stress state, with the transverse stress different from the longitudinal stress. The dielectric is subject to a radial stress at the surface. to be inﬁnite, and the longitudinal stress in the dielectric is zero. Inside the dielectric, the stress ﬁeld decays away from the hole. According to the Lame solution, the radial stress sr and the hoop stress sy in an inﬁnite elastic solid subject to a stress on a hole surface are given by (bib127 Timoshenko and Goodier, 1970) sr ðrÞ ¼ sT ða=rÞ2 ; sy ðrÞ ¼ sT ða=rÞ2 ; ð105Þ where r is the radial distance. Consequently, the stress ﬁeld in the composite is determined once sL and sT are determined. Next consider the strains. When the temperature changes by DT, the stresses change by DsT and DsL. The change in the longitudinal strain in the dielectric is caused by thermal expansion: DedL ¼ ad DT: ð106Þ On the hole surface, the radial and the hoop SX0716 CSI : 08125 Stress-Induced Voiding stresses in the dielectric are sr ¼ sT and sy ¼ sT. The change in the hoop strain is the sum of that caused by thermal expansion and that caused by the stresses: Dedy ¼ ad DT 1 þ nd DsT : Ed ð107Þ When we consider the strains in the metal, the analysis will depend on whether the metal has yielded. First assume that the metal is elastic. The changes in the strains in the metal are 1 2nm DsL DsT ; Em Em ð108Þ nm ð1 nm Þ DsL þ DsT : Em Em ð109Þ Dem L ¼ am DT þ Dem y ¼ am DT Because the metal and the dielectric are well bonded, so that the strains across the interface d m are compatible: DedL ¼ Dem L and Dey ¼ Dey : Solving two coupled linear algebraic equations, we obtain that ð1 þ nm Þðam ad ÞDT DsT ¼ ; ð110Þ ð1 þ nm Þð1 2nm Þ=Em þ ð1 þ nd Þ=Ed DsL ¼ Em ðam ad ÞDT þ 2nm DsT : ð111Þ When the metal and the dielectric have similar elastic constants, the stresses become DsT ¼ E ðam ad Þ DT; 2ð1 nÞ ð112Þ E ðam ad Þ DT: 1n ð113Þ DsL ¼ SX0720 So far we have assumed that the metal is elastic. For representative values, Em ¼ 1011 Pa, amad ¼ 20 106 K1, and DT ¼ 500 K, the stress is about 1 GPa, which exceeds typical yield strength of metals. We next allow the metal to yield plastically. Recall that the metal is under a triaxial stress state (sL, sT, sT). It is an empirical fact that superimposing a hydrostatic stress does not affect the plastic deformation of a metal. Imagine that we superimpose a hydrostatic state (sT, sT, sT) to the metal, so that the metal is under a uniaxial stress state (sLsT, 0, 0). We assume that metal is nonhardening, and the yield strength Y is independent of the temperature. One can readily modify the model to allow the yield strength to vary the temperature and strain, or even include the effect of creep. The metal and the dielectric are perfectly bonded. Consequently, the metal yield when the difference in the longitudinal and the transverse stress reaches 43 the yield strength: jsL sT j ¼ Y : ð114Þ After yielding, when the temperature changes, the two stresses can still change, provided they change by the same amount, DsL ¼ DsT. Let the plastic strain in the longitudinal direction be ep. Because plastic deformation conserves volume, the plastic strains in either of the two transverse directions must be ep/2. When the temperature changes by DT, after yielding, the strains in the metal change by p Dem L ¼ am DT þ De þ 1 2nm DsT ; Em 1 p 1 2nm Dem DsT : y ¼ am DT De þ 2 Em SX0725 ð115Þ ð116Þ The metal and the dielectric are bonded, so d m that DedL ¼ Dem L and Dey ¼ Dey : Solving for the transverse stress, we obtain that DsT ¼ 3ðam ad ÞDT : 3ð1 2nm Þ=Em þ 2ð1 þ nd Þ=Ed ð117Þ Note that this expression can be written as DsT ¼ 3Bðam ad ÞDT; with the effective elastic modulus given by (96). Figure 45 sketches the stress buildup as the temperature drops from the stress-free temperature T0. When the temperature is above a certain level, Te, the metal is elastic, and the stresses increase according to (110) and (111). The temperature Te is determined by inserting the stresses (110) and (111) into the yield condition (114), giving Figure 45 The stresses build up as the temperature drops. SX0730 CSI : 08125 44 Reliability of Interconnect Structures Em ðam ad ÞðT0 Te Þ Ed ð1 þ nm Þð1 2nm Þ : ¼1þ Y Em ð1 þ nd Þ ð118Þ At Te, the transverse stress is sT ðTe Þ ¼ SX0735 Ed ð1 þ nm Þ Y; Em ð1 þ nd Þ ð119Þ and the longitudinal stress is at a level Y above the transverse stress. As the temperature drops below Te, the stresses continue to build up, now with a different slope, given by (117). Figure 46 sketches the longitudinal stress as a function of temperature, assuming the metal to be elastic, or liquid-like, or elastic–plastic. At a given temperature below T0, the elastic metal acquires a high stress, and the liquid-like metal acquires a low stress. The stress in the elastic–plastic metal falls between the two limits. Because we assume that the yield strength Y is a constant, the two lines for the plastic and liquid-like metals are parallel. The longitudinal stress in the elastic–plastic metal line at temperature T is Ed ð1 þ nm Þ Y: sL ðTÞ ¼ 3Bðam ad ÞðT0 TÞ þ 1 þ Em ð1 þ nd Þ 8.7.5.4 Voiding in Blanket Copper Film bib109 Shaw et al. (2001) and bib107 Sekiguchi et al. (2001) have observed voids in blanket copper ﬁlms. In the experiment of Shaw et al., sketched in Figure 47, the copper ﬁlm was plated on SiO2 dielectric, and capped with a SiN layer. An annealing at 4001C closed all the voids, and left the copper ﬁlm under compression. The ﬁlm was then rapidly cooled and held at 2001C for 2 h; voids grew at the copper/nitride interface. Recall that SIV has been widely reported for encapsulated narrow aluminum lines, but not for blanket aluminum ﬁlms. As illustrated in Figure 48(a), in a blanket metal ﬁlm, creep can also relieve the biaxial stress by dislocation motion and atomic diffusion. Consequently, voiding (Figure 48(b)) must be regarded as a stress-relieving process in competition with creep. For a void to initiate from a small ﬂaw, the stress must be high enough to compete with the surface energy. The wafer curvature measurements have indicated that the stress in copper is typically higher than in aluminum, due mainly to the larger yield strength in copper ﬁlms (bib9 Baker et al., 2001; bib110 Shen et al., 1998). Furthermore, the elastic stiffness for copper is more anisotropic than aluminum. For a crystal of cubic symmetry, a ð120Þ The ﬁrst term is the hydrostatic tension in a liquid-like metal. The second term is due to the presence of the yield strength. A representative value of the yield strength at 2001C is 150 MPa, which contributes signiﬁcantly to the stress in the metal line. Figure 46 Compare stress in three cases: elastic metal, liquid-like metal, and elastic–plastic metal. Figure 47 When a blanket copper ﬁlm under tension is held at an elevated temperature, voids grow on the copper/nitride interface to relax the stress in the copper ﬁlm. Also sketched is the stress in the copper ﬁlm as the temperature cycles. SX0740 SX0745 CSI : 08125 Stress-Induced Voiding 45 Figure 48 Two processes to relieve stress in copper ﬁlm: (a) creep and (b) voiding. single number characterizes the degree of elastic anisotropy: x¼ AU:6 SX0750 C12 þ 2C44 : C11 ð121Þ For an isotropic elastic solid, x ¼ 1. Using the elastic constants listed in Section 8.7.5.2, one ﬁnds that x ¼ 1.1 for aluminum, and x ¼ 1.6 for copper. Finite element calculation has shown that the stress is high at the intersection of copper grain boundary and SiN cap layer (X. H. Liu, IBM, private communication). For the void to grow in size, atoms must diffuse from the void surface and plate on copper grain boundaries. The observation of voiding implies that creep is a less effective process to relieve the stress. This may be understood by comparing Figures 48(a) and (b). Assume that dislocations motions are constrained in the small volume. To relieve the stress in the copper ﬁlm, both creep and voiding require atoms to diffuse on the copper grain boundaries. In addition, creep requires that atoms diffuse on the copper/silica or copper/nitride interface, but voiding requires that atoms diffuse on the void surface. If the interface diffusion is slower than the surface diffusion, and if the grain boundary diffusion is not too much faster than the interface diffu- Figure 49 A void changes its shape (a) in an elastic solid, (b) on a grain boundary, and (c) in a viscous solid. sion, then voiding will be a more effective means to relieve stress than creep. After a long enough time, allowing atoms to diffuse on the interfaces, voids should disappear, driven by the surface energy, much like in powder sintering. Models of grain boundary diffusion in elastic solids (bib126 Thouless et al., 1996; bib35 Gao et al., 1999) can be adapted to model this phenomenon. 8.7.5.5 Slit-like Voids As illustrated in Figure 37, voids in an interconnect can have different shapes. A slitlike void signiﬁcantly increases electric resistance with a small amount of mass transport, and therefore may be responsible for earlier failure. Models of void shapes are brieﬂy considered here. Figure 49(a) illustrates a void of radius a in a crystal under remote stress s. SX0755 CSI : 08125 46 Reliability of Interconnect Structures For simplicity, we will only consider the uniaxial stress state. Assume that atomic transport inside the solid is much slower than on the void surface, so that the void can change shape as atoms relocate on its surface, and the solid is elastic. The surface energy favors a rounded void, but the elastic energy favors an elongated void. The stress at point A is higher than that at B, motivating atoms to diffuse on the surface. The relative importance of the elastic and the surface energy variations is expressed as a dimensionless number (bib116 Sun et al., 1994): s2 a : L¼ Eg SX0760 Next consider a single crystal under a uniaxial tension. A void in the crystal may change shape for several reasons. Elastic distortion causes small changes; large changes require mass transport. As illustrated in Figure 49(c), if the crystal creeps rapidly, the void elongates in the longitudinal direction (e.g., bib18 Budiansky et al., 1982). By contrast, if atoms diffuse rapidly on the void surface and the crystal is elastic, the void elongates in the transverse direction. 8.7.5.6 ð122Þ Under no stress, the void has a rounded shape maintained by the surface energy. When the crystal is under stress, two behaviors are expected. If the stress is small (L small), the void reaches an equilibrium shape close to an ellipse. If the stress is large (L larger), the void can never reach equilibrium; noses emerge and sharpen into crack tips. The critical value occurs at LcE1. Taking s ¼ 1 GPa; a ¼ 100 nm; E ¼ 70 GPa; and g ¼ 1 J m2 ; we ﬁnd from (122) that L ¼ 1.4. The mechanism operates only under very large stress. To place this mechanism into perspective, recall other mass transport mechanisms by which a void evolves. At elevated temperatures, surface tension and stress may relocate mass by diffusion on a surface and a grain boundary, and by diffusion and creep in a crystal lattice. First consider diffusion on surfaces and boundaries (Figure 49(b)). A void on a grain boundary normal to an applied tensile stress grows as atoms diffuse from the pore surface into the grain boundary (bib22 Chuang et al., 1979). When atoms diffuse faster on the grain boundary than on the void surface, the void cannot maintain the shape of spherical caps, and will become slit-like. Inserting one atom to the grain boundary, the tensile stress does work an amount given by Os. The elastic energy variation per atom relocation scales with Os2/Y. When atoms are mobile on the grain boundary, and the grains can drift relative to each other to accommodate the space, the elastic energy variation is much smaller than the work done by the stress associated with the insertion of atoms, Os2/ Y{Os. The effect of elasticity of the grains is negligible: the models assume rigid grains. However, when the grain boundary is absent, or atoms are immobile on the grain boundary, the tensile stress cannot do work, Os, and the elastic energy variation may become important. SX0765 The Effects of Low-k Dielectrics and Barriers A low-k dielectric often has a small elastic modulus and a large thermal expansion coefﬁcient. For example, SiLK has Young’s modulus 2.45 GPa and thermal expansion coefﬁcient 66 10–6 K1 (bib88 Martin et al., 2000). Will the metal line be under compression on cooling from the fabrication temperature? How small are the effective modulus B and the magnitude of the stress? Does the thin barrier layer between the metal and the dielectric play any role? Because different dielectrics will be used in coming years, it is important to have a convenient method to answer the above questions quantitatively (bib84 Ma et al., 1995; bib42 Hau-Riege and Thompson, 2000). Figure 50 illustrates the cross-section of several long metal lines embedded in a dielectric. In calculation, one can set the thermal expansion coefﬁcient of every material by its own value minus aSi. Because the Si substrate is bulky, the structure is under a state of plane strain deformation. The adjacent lines provide stiffness to each other. One can take a unit cell containing a single metal line, and prescribe zero displacement on the cell walls. Similar to Figure 47, remove the metal line from the structure, and leave behind a composite Figure 50 An interconnect structure on a silicon substrate, showing the metal lines, the barriers, and the dielectric. SX0770 SX0775 CSI : 08125 Electromigration structure of silicon, the dielectric, and the barrier layer. Apply a uniform normal traction s on the hole surface, and a temperature change DT. The structure is linear elastic, so that the change in the area of the cross-section is linear in the temperature change and the applied stress. Write 1 A Z un ds ¼ 2aeff DT s : meff SX0780 ð124Þ When the metal has no voids and is under a hydrostatic stress, the stress is given by s ¼ 3BDa(T0T). When the metal grows voids, and the stress in the metal is fully relieved, the SVV is given by Vsv ¼ 3Da(T0T)V. When the dielectric and the barrier have thermal expansion coefﬁcient similar to silicon, aeff ¼ 0, and (124) recovers (92). When the dielectric has a large thermal expansion coefﬁcient, and the barrier is negligibly thin, aeff will dominate (124). On cooling, the metal is under compression. The boundary value problem such as that in Figure 50 is easily solved by using the ﬁnite element method. To appreciate the trend, consider an idealized structure similar to that in Figure 44. The metal line has a circular cross-section of radius a, surrounded by a barrier of thickness hb, which in turn is surrounded by an inﬁnite dielectric. This problem can be solved analytically. The effective modulus meff relates to the shear modulus of the dielectric and the barrier: meff ¼ md þ mb hb =a; ð125Þ The effective thermal expansion coefﬁcient is aeff and a/hb ¼ 10, we obtain that meff ¼ 6.0 GPa. For copper interconnect, the barrier provides the effective modulus B ¼ 5.7 GPa. Even with a dielectric of negligible stiffness, the barrier itself can provide a signiﬁcant constraint. This fact has important implications for electromigration resistance, as described in the next section. ð123Þ The two coefﬁcients aeff and meff can be computed by solving the elasticity boundary value problem. The effective modulus B is still given by (96). The effective thermal expansion mismatch is 3Da ¼ 3ðam aSi Þ 2aeff : 47 md a ð1 þ nd Þðad aSi Þ þ ð1 þ nb Þðab aSi Þ mb hb : ¼ md a þ1 mb hb ð126Þ When (md/mb)(a/hb)c1, the dielectric prevails: meff ¼ md and aeff ¼ (1 þ nd)(adaSi). When (md/ mb)(a/hb){1, the barrier prevails: meff ¼ mbhb/a and aeff ¼ (1 þ nb) (abaSi). A representative set of magnitudes are md/mb ¼ 0.01, a/hb ¼ 10, (md/ mb)(a/hb) ¼ 0.1. When the barrier prevails, the saturation void volume is comparable to that in copper/silica structure. Taking mb ¼ 60 GPa 8.7.6 ELECTROMIGRATION In service, an interconnect line carries an intense electric current. The current motivates metal atoms to diffuse in the direction of electron ﬂow. The process, known as electromigration, has been the most menacing and persistent threat to interconnect reliability. Before this threat was recognized, electromigration had been one of the curious cross-ﬁeld transport phenomena, studied for its own sake (e.g., bib59 Huntington and Grone, 1961). The evolution of the electromigration research since the 1970s has been intertwined with that of the interconnect structure; see successive reviews coming out of the IBM T. J. Watson Research Center (bib27 d’Heurle and Rosenberg, 1973; bib26 d’Heurle and Ho, 1978; bib46 Ho and Kwok, 1989; bib51 Hu et al., 1995; bib104 Rosenberg et al., 2000). Since the early 1990s, as the mechanical effect on electromigration is better formulated (bib69 Korhonen et al., 1993), mechanics has become an integral part of the electromigration research. Stress both originates from, and affects, electromigration. There is no fundamental difference between the stress induced by thermal expansion mismatch and that induced by electromigration. Stress may open voids in the metal and break the encapsulation (bib21 Chiras and Clarke, 2000). Low-k dielectrics also have low stiffness, which signiﬁcantly inﬂuences electromigration (Lee et al., 2001; bib42 Hau-Riege and Thompson, 2000). As miniaturization continues, the diffusion time will be shorter. At least some of the interconnects will have to be designed to be immortal, on the basis of a stable state, rather than a transient process (bib117 Suo, 1998; bib6 Andleigh et al., 1999). This section focuses on issues speciﬁc to the reliability of encapsulated interconnect lines. As of early 2000s, the design of the interconnect structure is in a state of ﬂux. Materials, architectures, and processes will change. Models and experiments based on ﬁrst principles are particularly valuable in guiding future development. This section draws on the previous ones. In Sections 8.1.7.2 and 8.1.7.3 we consider cracking and debonding caused by SX0785 SX0790 AU:7 SX0795 CSI : 08125 48 Reliability of Interconnect Structures electromigration. Section 8.7.5 considers voiding caused by electromigration. Section 8.7.5.6 is particularly relevant when we consider the effects of low-k dielectrics. Even though Section 8.7.4, which is on ratcheting, dose not come in directly, the conscientious reader will soon feel the pains shared by the two widely used accelerated tests: thermal cycling and electromigration. Similarity will also be found in the models of the two phenomena. 8.7.6.1 SX0800 Electromigration in Encapsulated Metal Line Figure 51 illustrates an aluminum line encapsulated in a silica dielectric. The tungsten vias link aluminum lines between different levels. The titanium aluminide layers shunt the electric current where voids deplete a segment of aluminum. Figure 52 sketches the stress distribution along the metal line, assuming no voids. As the test temperature, the thermal expansion mismatch induces a triaxial tension in the aluminum line, as discussed in Section 8.7.5. At time t ¼ 0, subject the line to a direct electric current. Electrons enter the aluminum line from one tungsten via (cath- ode), and leave from another (anode). The electron ﬂow causes aluminum atoms to diffuse toward the anode. The atomic transport builds up tension near the cathode, and compression near the anode. The stress gradient promotes atoms to diffuse back to the cathode. After sometime, the interconnect reaches a steady state: the backﬂow balances the electromigration, and net atomic transport stops. The interconnect will last provided aluminum does not grow voids at cathode, or extrude at the anode. Next consider the case that the interconnect grows voids. Figure 53 summarizes the main observations. Thermal expansion misﬁt causes a tensile stress in aluminum. Each void grows and relaxes the stress in its vicinity (Figure 53(a)). After the line is subject to an electric current (Figure 53(b)), the voids exhibit extraordinarily complex dynamics: they disappear, re-form, drift, change shape, coalesce, and break up (bib87 Marieb et al., 1995). A particular behavior has captured much attention. A void sometimes takes the shape of a slit, lying inside a single grain, severing the metal line (bib105 Sanchez et al., 1992; bib103 Rose, 1992). bib7 Arzt et al. (1994) reported that a void is round initially; it moves, grows, and Figure 51 A schematic of an interconnect, embedded in a silicon dioxide matrix, on a silicon substrate. Figure 52 Schematic of the stress ﬁeld s(x, t) in an encapsulated metal line, assuming no voids. SX0805 CSI : 08125 Electromigration 49 Figure 53 (a) Upon cooling from the processing temperature, voids form to partially relaxed thermal stress. (b) Subject to a current, atoms diffuse toward the anode, and a void grows at the cathode end. (c) The line reaches the stable state, with a single void left at the cathode end, a linear pressure distribution in the rest of the line, and no further mass diffusion. Figure 54 Schematic of the stress ﬁeld s(x, t) in an encapsulated metal line, assuming that voids grow and move in the line. SX0810 then changes shape to become a slit. The void dynamics have been simulated (e.g., bib136 Wang et al., 1996; bib70 Kraft et al., 1997; bib142 Zhang et al., 1999). Despite the commotion in the transient, the end state is simple (bib32 bib33 Filippi et al., 1995, 2002). After a sufﬁciently long time, the metal line reaches a steady state (Figure 53(c)). Only a single void remains near the cathode; voids in the middle of the line have now been ﬁlled or swept into the cathode void. The total number of aluminum atoms is constant in the line. As the void at the cathode grows, atoms diffuse into the rest of the line, inducing a linear distribution of pressure (Figure 54). The pressure gradient balances the electron wind. The metal line behaves like a column of a liquid in the gravitational ﬁeld. The electron wind playing the role of gravity. Imagine several identical lines, each carrying a different current. Figure 55 illustrates the resistance change as a function of time. The resistance increases as the void enlarges. Two long-term trends are expected: the resistance either saturates or runs away. Evidently, the larger the current, the higher the saturation resistance. For a line carrying a large current, a large pressure gradient is needed to stop mass diffusion. The high pressure in the metal near the anode, in turn, may cause cracking or debonding in the encapsulation materials (bib21 Chiras and Clarke, 2000; bib75 Lee SX0815 CSI : 08125 50 Reliability of Interconnect Structures Figure 55 Resistance increases as a function of time. Under a small current, the resistance saturates. Under a large current, the resistance runs away. Figure 56 The aluminum line in the middle carries an electrical current in the direction perpendicular to the paper. The pressure in the aluminum line causes the silicon dioxide to crack, and aluminum to extrude (courtesy of W. K. Meyer). et al., 2002). Afterwards, the metal extrudes and the cathode void grows further, so that the resistance increases indeﬁnitely. Figures 56 and 57 show two examples of extrusion. The interconnect is immortal if a circuit tolerates a variable resistance in an interconnect up to its saturation level. 8.7.6.2 Basic Electromigration Characteristics (i) Electron Wind When a direct electric current ﬂows in a metal, the moving electrons impart momentum to metal atoms. The electron wind force per atom, fe, is proportional to the electric current SX0820 CSI : 08125 Electromigration Figure 57 Extrusion from an encapsulated aluminum line (courtesy of S. Chiras and D. R. Clarke). density j. Write (bib59 Huntington and Grone, 1961) fe ¼ Z erj; SX0825 ð127Þ where e is the electronic charge, and r the resistivity of the metal. Recall that rj is the electric ﬁeld in the metal line, and erj has the dimension of force. The dimensionless number Z* is known as the effective charge number. The sign convention makes Z*o0, because the electron wind force is in the direction of the electron ﬂow, opposite to that of the electric current density j. The electron wind force is small. When an atom moves by an atomic distance b, the work done by the force, feb, is much below the average thermal energy kT. Taking representaZ* ¼ 2, tive values b ¼ 1010 m, r ¼ 3 108 Om, j ¼ 1010 Am2, we ﬁnd that feb ¼ 5 108 eV. The average thermal energy is kT ¼ 0.04 eV at 500 K. Recall that the energy barrier for atomic motion in metals is on the order of 1 eV. Consequently, the electron wind causes metal atoms to diffuse. The atomic ﬂux is linearly proportional to the electron wind force. (ii) Atomic Diffusion SX0830 51 Einstein’s equation relates the atomic ﬂux J (i.e., the number of atoms crossing unit area per unit time) to the electron wind force: J¼ DZ erj ; OkT ð128Þ where D ¼ D0 exp(–Q/kT) is the diffusion coefﬁcient, Q is the activation energy, and O is the volume per atom in the metal. The equation is analogous to Equation (100) for diffusion motivated by the stress gradient. In a metal line, atoms may diffuse along several paths: the bulk crystal, the grain boundaries, the interface between the metal and the encapsulation, and the interface between the metal and the native oxide. Figure 58(a) sketches the cross-section of a wide metal line, width w, and thickness h. The metal line has columnar grains of diameter d. The effective Z*D, which enters (128) to give the total atomic ﬂux, results from all three kinds of paths (bib52 Hu et al., 1999): 1 d 1 Z D ¼ ZB DB þ ZG DG dG d w 1 1 þ ; þ 2ZI DI dI w h ð129Þ where the subscripts B, G, and I signify the bulk, the grain boundary, and the interface; dG and dI are the width of the grain boundary and the interface, respectively. The melting temperatures of aluminum and copper are 933 K and 1358 K, respectively. The temperatures at which electromigration is of concern are below 500 K. For ﬁne metal lines, bulk diffusion is SX0835 CSI : 08125 52 Reliability of Interconnect Structures Figure 59 Schematic of the edge drift experiment. Figure 58 (a) The cross-section of a wide metal line. (b) A narrow line with a bamboo grain structure. negligible. When a metal line is narrow, the grains form a bamboo structure, with all the grain boundaries perpendicular to the ﬂux direction (Figure 58(b)). For such a bamboo line, the grain boundaries do not contribute to the mass transport; the only remaining diffusion path is the interfaces. As miniaturization continues, a large fraction of atoms will be on the interfaces, so that the effective diffusivity will increase (Equation (129)). (iii) Median Time-to-Failure SX0840 SX0845 The most widely used method to characterize electromigration is to measure the median time-to-failure (MTF). Subject a batch of lines to a known current density and temperature. The lines grow voids. When a void severs a line, the current stops and the line fails. Due to the statistical nature of void formation, failure times scatter even for a batch of carefully processed lines. The MTF is taken as the time at which 50% of the lines have failed. In the interconnect structure with shunt layers, voids never stop the current. A line is taken to have failed when the resistance increases by, say, 20%. MTF measurements provide a convenient way to evaluate effects of various parameters on electromigration. For example, it has been shown that Al lines containing a few percent of Cu last about 80 times longer than pure Al lines (bib5 Ames et al., 1970), that intermetallic shunts greatly increase electromigration resis- tance (bib48 Howard et al., 1978), that narrow Al lines of bamboo grain structures last longer than polycrystalline wide Al ﬁlms (bib129 Vaidya et al., 1980), and that Cu lines last longer than Al lines (bib104 Rosenberg et al., 2000). To fail lines within a time suitable for laboratory measurements, one has to accelerate the test by using temperatures and electric current densities higher than those used in service. The MFT can be measured for several temperatures and current densities. The results are ﬁt to an empirical relation (bib13 Black, 1969): Q ; MFT ¼ Aj n exp kT SX0850 ð130Þ where A, n, and Q are ﬁtting parameters. The exponent n typically ranges between 1 and 2. The activation energy Q determined in this way is consistent with that determined by other methods. The use of MFT to project service lifetime raises at least two objections. First, the values of MFT are measured under accelerated conditions. Any conclusion drawn by extrapolation to the service condition is suspect. Second, the interconnect structure has little redundancy. The whole structure fails by the earliest failure of a small number of lines. Valid measurements of the low-percentage-failure tail of the time-to-failure curve involve large numbers of samples (bib34 Gall et al., 2001). SX0855 (iv) Line Edge Drift Another useful experiment involves line edge drift. In their original experiment, bib15 Blech and Kinsbron (1975) deposited a gold ﬁlm on a molybdenum ﬁlm, which in turn was deposited on an oxide-covered silicon wafer (Figure 59). Molybdenum served as the electrodes. Because SX0860 CSI : 08125 Electromigration SX0865 molybdenum has much higher resistance than gold, in the molybdenum/gold bilayer, the electric current mainly ﬂew in gold. Gold atoms diffused in the direction of the electron ﬂow. The edge of the gold ﬁlm at the cathode drifted, and atoms piled up at anode edge. The edge of the gold ﬁlm drifted at a constant velocity at a given current and temperature. The drift velocity v relates to the atomic ﬂux as v ¼ OJ. Using (128), one expresses the drift velocity as v¼ DZ erj : kT ð131Þ Rewrite the above equation as ln SX0870 SX0875 ð132Þ It is convenient to plot the experimentally measured ln (vT/j) as a function of 1/T. The data points often fall on a straight line. The slope of the line determines the activation energy Q, and the intercept determines the product D0Z*. An additional independent experiment is needed to separate D0 and Z*. We will discuss such experiments later. Compared to the MTF measurements, the drift velocity measurements require the observation of the edge displacement. In return, the drift velocity measurements provide the values of D0Z*. Furthermore, the drift velocity does not have the large statistical scatter associated with void formation. In principle, a single sample can be used to measure the drift velocities at various temperatures. Such measurements are sufﬁcient to determine Q and D0Z*. The drift experiment has been used to determine the dominant diffusion paths for aluminum (bib53 Hu et al., 1993) and copper (bib52 Hu et al., 1999; bib81 Liniger et al., 2002). It has been used to study alloying effects in copper lines (bib76 Lee et al., 1995). The drift experiment led bib14 Blech (1976) himself to discover a quantitative mechanical effect on electromigration. This landmark discovery has since become a guiding light in the interconnect structure design and electromigration research. The remainder of the section describes this discovery and its consequences. 8.7.6.3 SX0880 vT D0 Z er Q ¼ ln : j k kT Balancing Electron Wind with Stress Gradient On measuring the drift velocity in an aluminum line, bib14 Blech (1976) found that the line edge drifted only when the current density was above a threshold value. He tested lines between 30 mm and 150 mm long. The 53 threshold current density was inversely proportional to the line length. The product of the line length L and the threshold current density jc was a constant, jc L ¼ 1:26 105 A m1 : The jcL product increased when the aluminum lines were encapsulated in SiN. Blech attributed the observations to the pressure buildup near the anode. The pressure buildup in aluminum was evident as it sometimes cracked the overlying SiN. The pressure also caused a long aluminum extrusion through a hole etched in the SiN near the anode. Blech used aluminum lines 25 mm wide and 0.46 mm thick, with columnar grains. Such wide ﬁlms could develop biaxial stresses, but not triaxial stresses. Atoms left the cathode region, where tension arose. Atoms arrived in the anode region, where compression built up. At a point in the line, atoms diffuse along the grain boundaries to equalize the two in-plane stress components. The in-plane stresses could not be readily relaxed because diffusion on the aluminum–oxide interfaces is negligible. The stress gradient drove atoms to diffuse from the anode (in compression) to cathode (in tension). The direction was opposite to the electron wind. When the stress gradient balanced the electron wind, net atomic diffusion stopped. Incidentally, bib15 Blech and Kinsbron (1975) did not report any threshold current density for gold lines. Presumably, diffusion on gold surface was so fast that the gold ﬁlm could not build up signiﬁcant stresses during the electromigration experiment. Denote the equal biaxial stress by s, which is a function of the position x along the line and time t. An atom in the metal line is subject to both the electron wind and the stress gradient. The net force is the sum of (99) and (127), namely, f ¼ Z erj þ O qs : qx ð133Þ The evolution of the stress ﬁeld s(x, t) will be discussed later. We now focus on the steady state. After a sufﬁciently long time, the net atomic diffusion stops, and the net driving force vanishes, f ¼ 0. From (133), the line reaches the steady state when the stress in the line has a constant slope, so that the stress needed to balance the electron wind force is ODs ¼ Z erjL; ð134Þ where Ds is the stress difference between the two ends of the line. For a very small current, the steady stress Ds is small. Wide aluminum lines have ﬁnite yield strength, which has been determined by the wafer curvature measurements (bib95 Nix, 1989). The lines drift when SX0885 SX0890 CSI : 08125 54 SX0895 the stresses at both ends exceed the yield strength. Take O ¼ 1.66 1029 m3, Z* ¼ 2, r ¼ 3 108 Om, Ds ¼ 108 Pa, and we ﬁnd that jcL ¼ 1.73 105 Am1. The mechanical constraint effect on electromigration lifetime had been reported before Blech’s work. For example, bib1 Ainslie et al. (1972) developed Equation (134) to estimate the stress needed to stop electromigration. These authors used a value Z* ¼ 60 in their estimate, and found an extremely large stress, which could not be sustained by the encapsulation. They abandoned this interpretation, and instead tried to explain the mechanical effect in terms of the effect of stress on diffusivity. The Blech experiment eliminated any diffusivityrelated interpretation, because diffusion stopped when the current was below the threshold. Indeed, once the threshold current is measured, together with the yield strength measured by the wafer curvature method, Equation (134) determines the value of Z*, without being convoluted with the diffusivity. 8.7.6.4 SX0900 SX0905 Reliability of Interconnect Structures No-Voiding Condition for Encapsulated Line We now return to Figure 52 for a quantitative discussion. On cooling from the stress-free temperature T0 to a temperature T, the metal line and the encapsulation have a mismatch volumetric strain 3Da(T0T). When the structure is held at T for a sufﬁciently long time, the line will evolve into one of the two equilibrium states: either a uniform hydrostatic stress state s ¼ 3Da(T0T)B with no voids, or a stress-free state with a saturated void volume, SVV ¼ 3Da(T0T)V. Here V is the volume of the metal line. Section 8.7.5.6 prescribes ways to calculate the effective thermal expansion coefﬁcient mismatch Da and elastic modulus B. The evolution is facilitated by atomic transport. At a ﬁnite time, the metal line is in a transient state. The stress state is nonhydrostatic and nonuniform. Voids and unrelaxed metal coexist. Of the two equilibrium states, the hydrostatic state is metastable, but the state with SVV is stable. Consider the hydrostatic state ﬁrst. In Figure 52, this hydrostatic stress ﬁeld is labeled as t ¼ 0. Section 8.7.5.2 prescribes a critical stress for void initiation, svoid ¼ 2g/a, where a is the radius of the pre-existing ﬂaw size, and g the surface energy. The condition can be modiﬁed for ﬂaws on interfaces, or junctions between the grain boundaries and the interfaces. It is assumed that the annealing will close all voids provided the uniform hydrostatic stress is below the critical stress, sosvoid. For a copper/low-k structure, taking T0T ¼ 200 K, Da ¼ 13 106 K1, B ¼ 6 109 Pa, g ¼ 1 Jm2 and a ¼ 5 nm, we ﬁnd that the hydrostatic stress is s ¼ 0.47 108 Pa, and the critical stress is svoid ¼ 4 108 Pa. This comparison seems to suggest that the compliant dielectrics reduce B, making the stress-induced voiding less likely. The above void initiation condition is overly simplistic, and is risky. It assumes an artiﬁcial scenario: the metal reaches the hydrostatic state ﬁrst, and then the ﬂaws start to question themselves whether to enlarge or shrink. In reality, during annealing, the elastic anisotropy between metal grains, as well as the elastic inhomogeneity between the metal and the encapsulation, can momentarily cause very high stresses at various junctions. If atomic transport is slow in relaxing the metal into the hydrostatic state, the high stresses may cause the ﬂaws to grow. The situation is worse than voiding in blanket ﬁlms discussed in Section 8.7.5.4. A stress-free and void-free blanket ﬁlm is the stable equilibrium state. By contrast, in an encapsulated metal line, the uniform hydrostatic state is only metastable; the voids, once initiated, will grow until the entire line is stress free. Experiments of bib41 Hau-Riege (2001) showed that voids formed in copper lines even at very small electric current. With caution, we pursue this risky model further, asking whether a superimposed electric current will initiate voiding. After the electric current is applied, the metal line evolves to a steady state, in which the stress is linearly distributed. The number of atoms is conserved in the metal line. If no voids form, atoms lost in the cathode region relocate to the anode region. By symmetry, the middle of the line neither loses nor gains atoms, and remains to have the stress, s(L/2, t) ¼ 3Da(T0T)B, at all time. The steady stress state as t-N in the line is sðx; NÞ ¼ 3DaðT0 TÞB SX0915 Z erj L x : ð136Þ O 2 In Figure 52, this steady state stress ﬁeld is labeled as t ¼ N. We assume that voids do not initiate if the steady stress at the cathode is below the critical stress, s(0, N)osvoid, namely, 3DaðT0 TÞB þ SX0910 Z er jLosvoid : 2O ð137Þ Figure 60 sketches this condition on the plane spanned by the temperature T and the product jL. On this plane, Equation (137) is the straight line. Below the straight line, the current density is low and the temperature is high, so voids will SX0920 CSI : 08125 Electromigration 55 contributions, the SVV is (bib69 Korhonen et al., 1993; bib117 Suo, 1998) Vsv Z er jL: ¼ 3DaðT0 TÞ þ 2OB V Figure 60 The product jcL as a function of temperature. not form. Above the straight line, the void will form. 8.7.6.5 SX0925 Saturated Void Volume (SVV) A conservative model assumes that the voids grow in the metal line (Figure 53). Figure 54 sketches the stress evolution in such a metal line. Before the line carries the electric current, voids may already grow in the line due to thermal stresses. This stress distribution is labeled as t ¼ 0 in Figure 54. After the line carries the electric ﬁeld for sometime, all the voids along the line disappear, and a single void is left in the cathode edge. The void relieves the stress at the cathode, s(0, t) ¼ 0; the capillary pressure is negligible. The stress at the anode becomes compressive. When the stress gradient balances the electron wind, the stress is linearly distributed along the line: sðx; NÞ ¼ Z erjx=O; SX0930 ð138Þ This stress distribution is labeled as t ¼ N in Figure 54. The steady stress ﬁeld is unaffected by the temperature, to the extent that the temperature dependence of the material constants in (138) are negligible. In contrast to the void-free steady state (136), the steady state with a cathode void is stable. No further change will occur in the line until the current density or the temperature changes. The void at the cathode end reaches the saturated volume. The thermal expansion mismatch contributes 3Da(T0T)V to the SVV. R L The steady stress ﬁeld s contributes A 0 ðs=BÞ dx to the SVV, where A is the crosssectional area of the metal line. Adding the two ð139Þ The SVV increases when the temperature decreases and the current density increases. The void volume affects the resistance increase, as discussed in Section 8.7.5.2. Failure can be set to the condition that Vsv/V reaches a critical value. On the plane spanned by T and jL, Equation (139) appear the same as that shown on Figure 60, but with the intercept replaced by T0(Vsv/ V)/(3Da). The slope of the line is proportional to B. Everything else being equal, jcL increases with B. In Section 8.7.5.6, we estimated that when the encapsulation changes form Ta/silica to Ta/SiLK, the effective modulus drops by about a factor of 4. Lee et al. (2002) have found that jcL ¼ 3.7 A m1 and 1.2 105 A m1 for the two kinds structures, respectively. When the temperature drops, the thermal stress increases, and the critical current density decreases. The slope of the straight line in Figure 60 is 6OBDa/|Z*er|. An estimate gives the value of this slope to be 2 103 A m1 K1. That is, decreasing the temperature by 100 K, one expects a decrease of the jcL product by 2 105 A m1. This decrease may be of practical concern, because jcL is measured at an elevated temperature in an accelerated test, and is often reported without qualiﬁcation. I am unaware of any experimental support for this trend. Incidentally, in bib14 Blech’s (1976) drift experiment, jcL increased as the temperature dropped from 500 K to 200 K. He used wide aluminum lines. The high values of jcL at low temperatures should be due to the corresponding high yield strength. In writing (139), we have ignored the volume change due to the chemical reaction between aluminum and titanium. Any volume expansion associated with such a reaction would reduce the saturation void volume. Similarly, encapsulation materials leading to a small or even negative Da will reduce the SVV. The copper interconnect structures in use have very thin barrier layers. They are ineffective as shunts: the resistance abruptly increases when a void at the cathode grows across the via (bib41 Hau-Riege, 2001; bib135 Wang and Filippi, 2001). A more appropriate failure criterion should be the void volume Vsv itself, rather than the volumetric strain Vsv/V, reaching a critical value. Neglecting the thermal strain in (139), one ﬁnds that VsvpjL2/B. bib41 Hau-Riege (2001) has suggested that jL2/B, instead of jL, be used as a ﬁgure of merit. The SX0935 SX0940 SX0945 SX0950 CSI : 08125 56 Reliability of Interconnect Structures void-at-via problem can be mitigated by methods to generate a void off the via, at a location uncritical to the interconnect (bib50 Hu et al., 2001). Of course, it remains an option to provide a low-resistance shunt to the interconnect structure. 8.7.6.6 SX0955 SX0960 SX0965 Experimental Determination of Z ; DaðT T0 Þ; B; and D No reliable method exists to compute Z* from ﬁrst principles; the parameter is measured experimentally. There has been progress in computing diffusivity D form ﬁrst principles; however, interconnects have multiple diffusion paths, and computations involving interfaces and grain boundaries are unreliable. Although one can compute Da and B as described in Section 8.7.5.6, it is desirable to measure such important parameters experimentally, especially when input material parameters needed for computation are unreliable. As discussed above, the drift experiment with unpassivated lines gives the product Z*D. Additional independent experiments are needed to separate them, and to determine B and Da. Void in encapsulated metal lines can be observed in situ using high-voltage scanning electron microscopy (bib87 Marieb et al., 1995). When the void at the cathode is large enough, its growth can be observed as the displacement of line edge at the cathode, similar to the original bib15 Blech–Kinsbron (1975) drift velocity experiment. Figure 61 plots the SVV as a function of the jL product, as predicted by Equation (139). If the saturation void volume is measured experimentally at several current densities, the slope of the line in Figure 61 determines the ratio Z*/B, and the intercept gives 3Da(T0T). Figure 62 sketches the void volume as a function of time. After the line attains the steady state, one can stop the electric current. The stress gradient in the line will drive atoms to diffuse back, and the void will shrink. The same line can be tested at various current densities and temperatures. Similar to the stress relaxation described in Section 8.7.5.2, the process of approaching steady state is governed by a diffusion equation. Both the electron wind and the pressure gradient drive the atomic ﬂux: D @s Z erj þ O : J¼ OkT @x ð140Þ The diffusivity is taken to be an average in the aluminum line. Inserting (140) into (101) leads to the diffusion equation (102) for the stress ﬁeld s(x, t). The solution to this classical initial-boundary value problem takes the form Figure 61 The normalized saturation void volume as a function of the jL product. Figure 62 The normalized void volume, as a function of time, ﬁrst approaches the saturation under a current, and then relaxes to the thermal misﬁt volume after the current is stopped. of an inﬁnite series, the slowest decaying term being proportional to exp (–t/t), with t¼ L2 kT : p2 DBO ð141Þ Note that the timescale is independent of the current density. A large current density transports mass at a high rate, but also needs to transport more mass to reach the steady state. An experimental measurement of the relaxation time determines the product DB. In combination with the Z*/B measured by the saturation volume, and Z*D by the edge drift of a line with encapsulation of negligible stiffness, one can separate the three parameters Z*, D, and B. The number Z* can also be determined, on the basis of the steady stress distribution (138), by measuring the stress in the metal line using synchrotron-based X-ray microdiffraction (bib134 Wang et al., 1998), or by measuring SX0970 CSI : 08125 Electromigration the fringe stress ﬁeld in silicon using Raman spectroscopy (bib84 Ma et al., 1995). 8.7.6.7 SX0975 No-Extrusion Condition for Encapsulated Line In the steady state with SVV, the compressive stress in the metal line at the anode is sA ¼ Z erjL=O: SX0980 Using L ¼ 100 mm, j ¼ 1.0 1010 Am2, Z* ¼ 2, r ¼ 3 108 Om, and e ¼ 1.6 1019 C, –29 3 O ¼ 1.66 10 m , one ﬁnds that the steadystate compressive stress at the anode is sA ¼ 600 MPa. The large stress may cause cracking or debonding of the encapsulation. For example, bib32 Filippi et al. (1995) tested 100 mm aluminum lines under various current densities, and reported that aluminum did not extrude under 0.56 1010 A m2, but did under 1.0 1010 A m2. Section 8.7.2.2 has outlined the application of fracture mechanics to structures of small feature size. The fabrication process controls the geometry all the way to the feature size, so that crack-like ﬂaws must be smaller than the feature size. Use the linewidth, w, as a representative size scale, the no-extrusion condition is stated as (bib117 Suo, 1998) b SX0985 ð142Þ s2A w oG; E ð143Þ Here G is the fracture energy of the encapsulation material or the interface, E the Young’s modulus of the material, and b a dimensionless parameter depending on ratios of various elastic moduli and lengths that describe the anode. The values of b can be calculated by solving the elasticity boundary value problems containing cracks. Taking representative values such as b ¼ 0.25, G ¼ 4 Jm2, E ¼ 70 GPa, and w ¼ 0.5 mm, one ﬁnds from (2) that the encapsulation can sustain anode pressure up to |sA| ¼ 1.5 GPa. In the above, thermal stresses in the passivation have been ignored. Upon cooling from the processing temperature, a large compressive hoop stress arises in the oxide, resulting from the thermal expansion misﬁts between the aluminum and the oxide, and between the silicon substrate and the oxide. When an electric current is supplied, the volume of aluminum near the anode increases, which ﬁrst compensates its thermal contraction, and then goes beyond. Consequently, in the stable state, the stress in the oxide is due to the pressure in the aluminum, and the thermal misﬁt between 57 the oxide and the silicon substrate. The latter is negligible. Two other circumstances should be mentioned in this connection. Some dielectrics may develop large intrinsic stresses at the deposition temperature. They are unrelated to the volume change of aluminum, and persist under temperature change and current. A second circumstance involves a line tested under a current up to the stable state, and then brought to a higher temperature. Instantaneously, the thermal expansion misﬁt between aluminum and oxide adds more tensile stress in the insulator. In such cases, the additional stresses must be included in the no-extrusion condition. Compliant low-k dielectrics present a new challenge. As a ﬁrst approximation, we model the Ta barrier as a cylindrical pressure vessel of radius a and thickness hb, and neglect the dielectric. The hoop stress in the barrier sy relates to the internal pressure sA as sy ¼ |sA|a/ hb. Assume that crack-like ﬂaw size is on the order of the barrier thickness hb. The noextrusion condition may be written as b s2A a2 oG: Ehb SX0995 ð144Þ The above estimates are intended to illustrate a basic modeling approach. Because the structural details at line ends are complicated, accurate calculation is difﬁcult. A more reliable method is to carry out experiments with known current density, and use the electromigration generated stress to test the condition for extrusion (bib21 Chiras and Clarke, 2000). 8.7.6.8 SX0990 SX1000 The Immortal Interconnect Provided a circuit tolerates a variable resistance in an interconnect up to its saturation level, the interconnect is immortal (bib117 Suo, 1998; bib6 Andleigh et al., 1999). The interconnect evolves into a stable state to adapt to the newly established temperature and current. The immortality gives a simple perspective on reliability. One can focus on the stable state itself, rather than the transient process to reach it. The perspective plays down the roles of the timescale, the rate processes, and the microstructure of the metal. No longer need the microstructure be optimized for slow mass transport or low void nucleation rate. No longer need the MTF be measured, for the lifetime is inﬁnite. No longer need a magic alloy be sought to slow down diffusion rate, for the diffusivity is irrelevant. In short, the reliability is warranted by energetics, rather SX1005 CSI : 08125 58 SX1010 SX1015 Reliability of Interconnect Structures than kinetics. Having thermodynamics on our side, the design is much more robust. The use of the stable state is limited in two ways: the metal may extrude at the anode, or the saturation resistance may be prohibitively large. For a short line, the saturation void volume is small compared to the via size, giving rise to a small change in resistance. Consequently, the stable state ﬁnds ready applications in short lines. The saturation void volume increases when the effective modulus B is small (Equation (139)). The interconnect structure with low-k dielectrics and thin barriers no doubt require attention. The copper interconnect structures in use have very thin barrier layers. They are ineffective as shunts: the resistance abruptly increases when a void at the cathode grows across the via. An immortal interconnect would require low-resistance shunts. As miniaturization continues, larger fraction of atoms will be on the metal/encapsulation interface. The effective diffusivity will be larger (Equation (129)), and the diffusion time shorter. The day may arrive when some of the interconnects must be designed to be immortal. Investigation into ways to limit the resistance increase and to prevent metal extrusion will prepare us for such a day. ACKNOWLEDGMENTS SX1016 The work of my group in this area has been supported over the years by the National Science Foundation, Ofﬁce of Navel Research, Defense Advanced Research Projects Agency, New Jersey Science and Technology Commission, Institute for Materials Research and Engineering, and Intel Corporation. Dr. Z. Y. Huang has kindly helped me prepare the ﬁgures. REFERENCES bib1 bib2 bib3 AU:8 bib4 bib5 N. G. Ainslie, F. M. d’Heurle and O. C. Wells, 1972, Coating, mechanical constraints, and pressure effects on electromigration. Appl. Phys. Lett., 20, 173–174. P. Alpern, V. Wicher and R. Tilgner, 1994, A simple test chip to assess chip and package design in the case of plastic assembling. IEEE Trans. Compon. Pack. Manuf. Technol. A, 17, 583–589 (correction in 1995, 18, 862– 863). J. M. Ambrico and M. R. Begley, 2002, The role of initial ﬂaw size and plasticity in adjacent layers in channeling crack growth in thin ﬁlms, submitted. J. M. Ambrico, E. E. Jones and M. R. Begley, 2002, Cracking in thin multi-layers with ﬁnite width and periodic architectures. Int. J. Solids Struct., 39, 1443– 1462. I. Ames, F. d’Heurle and R. Horstmann, 1970, Reduction of electromigration in aluminum ﬁlms by copper doping. IBM J. Res. Develop., 14, 461–463. V. K. Andleigh, V. T. Srikar, Y. J. Park and C. V. Thompson, 1999, Mechanism maps for electromigration-induced failure of metal and alloy interconnects. J. Appl. Phys., 86, 6737–6745. E. Arzt, O. Kraft, W. D. Nix and J. E. Sanchez, 1994, Electromigration failure by shape change of voids in bamboo lines. J. Appl. Phys., 76, 1563–1571. A. Bagchi, G. E. Lucus, Z. Suo and A. G. Evans, 1994, A new procedure for measuring the decohesion energy for thin ductile ﬁlms on substrate. J. Mater. Res., 9, 1734– 1741. S. P. Baker, A. Kretschmann and E. Arzt, 2001, Thermomechanical behavior of different texture components in Cu thin ﬁlms. Acta Mater., 49, 2145–2160. M. R. Begley and A. G. Evans, 2001, Progressive cracking of a multilayer system upon thermal cycling. J. Appl. Mech., 68, 513–520. J. L. Beuth, 1992, Cracking of thin bonded ﬁlms in residual tension. Int. J. Solids Struct., 29, 1657–1675. J. L. Beuth and N. W. Klingbeil, 1996, Cracking of thin ﬁlms bonded to elastic–plastic substrates. J. Mech. Phys. Solids, 44, 1411–1428. J. R. Black, 1969, Electromigration—a brief survey and some recent results. IEEE Trans. Electron Devices, ED16, 338–347. I. A. Blech, 1976, Electromigration in thin aluminum ﬁlms on titanium nitride. J. Appl. Phys., 47, 1203–1208. I. A. Blech and E. Kinsbron, 1975, Electromigration in thin gold ﬁlms on molybdenum surfaces. Thin Solid Films, 25, 327–334. I. A. Blech and E. S. Meieran, 1967, Direct transmission electron microscope observation of electrotransport in aluminum thin ﬁlms. Appl. Phys. Lett., 11, 263–265. J. Bree, 1967, Elastic–plastic behaviour of thin tubes subjected to internal pressure and intermittent high-heat ﬂuxes with application to fast-nuclear-reactor fuel elements. J. Strain Analysis, 2, 226–238. B. Budiansky, J. W. Hutchinson and S. Slutsky, 1982, Void growth and collapse in viscous solids. In: ‘‘Mechanics of Solids, The Rodney Hill 60th Anniversary Volume,’’ eds. H. G. Hopkins and J. Sewell, Pergamon Press, Oxford, pp. 13–45. H. C. Cao and A. G. Evans, 1989, An experimental study of the fracture resistance of bimaterial interface. Mech. Mater., 7, 295–305. P. G. Charalambides, J. Lund, A. G. Evans and R. M. McMeeking, 1989, A test specimen for determining the fracture resistance of bimaterial interfaces. J. Appl. Mech., 56, 77–82. S. Chiras and D. R. Clarke, 2000, Dielectric cracking produced by electromigration in microelectronic interconnects. J. Appl. Phys., 88, 6302–6312. T.-J. Chuang, K. I. Kagawa, J. R. Rice and L. B. Sills, 1979, Non-equilibrium models for diffusive cavitation of grain interfaces. Acta Metall., 27, 265–284. R. F. Cook and E. G. Liniger, 1999, Stress-corrosion cracking of low-dielectric-constant spin-on-glass thin ﬁlms. J. Electochem. Soc., 146, 4439–4448. J. Curry, G. Fitzgibbon, Y. Guan, R. Muollo, G. Nelson and A. Thomas, 1984, New failure mechanisms in sputtered aluminum–silicon ﬁlms. In: ‘‘22nd Ann. Proc. IEEE Int. Reliability Phys. Symp.,’’ pp. 6–8. R. H. Dauskardt, M. Lane, Q. Ma and N. Krishna, 1998, Adhesion and debonding of multi-layer thin ﬁlm structures. Eng. Fract. Mech., 61, 141–162. F. M. d’Heurle and P. S. Ho, 1978, Electromigration in thin ﬁlms. In: ‘‘Thin Films: Interdiffusion and Reactions,’’ eds. J. Poate, K. N. Tu and J. Mayer, Wiley, New York, pp. 243–303. F. M. d’Heurle and R. Rosenberg, 1973, Electromigration in thin ﬁlms. In: ‘‘Physics of Thin Films,’’ eds. G. Hass, M. Francombe and R. Hoffman, Academic Press, New York, vol. 7, pp. 257–310. bib6 bib7 bib8 bib9 bib10 bib11 bib12 bib13 bib14 bib15 bib16 bib17 bib18 bib19 bib20 bib21 bib22 bib23 bib24 AU:9 bib25 bib26 bib27 CSI : 08125 Electromigration bib28 bib29 bib30 bib31 bib32 bib33 bib34 bib35 bib36 bib37 bib38 bib39 bib40 bib41 AU:10 bib42 AU:11 bib43 bib44 AU:12 bib45 bib46 bib47 AU:13 D. R. Edwards, K. G. Heinen, S. K. Groothuis and J. E. Martinez, 1987, Shear-stress evaluation of plastic packages. IEEE Trans. Compon. Hybrids Manuf. Technol., 12, 618–627. F. Erdogan and G. C. Sih, 1963, On the crack extension in plates under plane loading and transverse shear. J. Basic Eng., Trans. ASME, 85, 519–527. A. G. Evans, M. D. Drory and M. S. Hu, 1988, The cracking and decohesion of thin ﬁlms. J. Mater. Res., 3, 1043–1049. A. G. Evans and J. W. Hutchinson, 1995, The thermomechanical integrity of thin ﬁlms and multilayers. Acta Metall. Mater., 43, 2507–2530. R. G. Filippi, G. A. Biery and R. A. Wachnik, 1995, The electromigration short-length effect in Ti–AlCu–Ti metallization with tungsten studs. J. Appl. Phys., 78, 3756–3768. R. G. Filippi, R. A. Wachnik, C.-P. Eng, D. Chidambarrao, P.-C. Wang, J. F. White, M. A. Korhonen, T. M. Shaw, R. Rosenberg and T. D. Sullivan, 2002, The effect of current density, stripe length, stripe width, and temperature on resistance saturation during electromigration testing. J. Appl. Phys., 91, 5787–5795. M. Gall, C. Capasso, D. Jawaranl, R. Hemandez, H. Kawasaki and P. S. Ho, 2001, Statistical analysis of early failures in electromigration. J. Appl. Phys., 90, 732–740. H. Gao, L. Zhang, W. D. Nix, C. V. Thompson and E. Arzt, 1999, Crack-like grain-boundary diffusion wedges in thin metal ﬁlms. Acta Mater., 47, 2865–2878. S. A. Gee, M. R. Johnson and K. L. Chen, 1995, A test chip design for detecting thin-ﬁlm cracking in integratedcircuits. IEEE Trans. Compon. Pack. Manuf. Technol. B, 18, 478–484. A. Gouldstone, Y. L. Shen, S. Suresh and C. V. Thompson, 1998, Evolution of stresses in passivated and unpassivated metal interconnects. J. Mater. Res., 13, 1956–1966. B. Greenebaum, A. I. Sauter, P. A. Flinn and W. D. Nix, 1991, Stress in metal lines under passivation—comparison of experiment with ﬁnite-element calculations. Appl. Phys. Lett., 58, 1845–1847. C. K. Gurumurthy, J. Jiao, L. G. Norris, C.-Y. Hui and E. J. Kramer, 1998, A thermo-mechanical approach for fatigue testing of polymer bimaterial interfaces. ASME Trans. J. Electron. Packag., 120, 372–378. J. B. Han, 2001, Flip-chip BGA design to avert die cracking. J. Electron. Packag., 123, 58–63. S. P. Hau-Riege, 2001, Immortality of Cu damascene interconnects. In: ‘‘6th International Workshop on Stress-induced Phenomena in Metallization,’’ eds. S. P. Baker, M. A. Korhonen, E. Arzt and P. S. Ho, Am. Inst. Phys., pp. 21–32. S. P. Hau-Riege and C. V. Thompson, 2000, The effects of the mechanical properties of the conﬁnement material on electromigration in metallic interconnects. 15, 1797– 1802. M. Y. He, A. G. Evans and J. W. Hutchinson, 2000, The ratcheting of compressed thermally grown thin ﬁlms on ductile substrates. Acta Mater., 48, 2593–2601. R. Hill, 1950, ‘‘The Mathematical Theory of Plasticity,’’ Clarendon Press, Oxford. K. Hinode, I. Asano, T. Ishiba and Y. Homma, 1990, A study on stress-induced migration in aluminum metallization based on direct stress measurements. J. Vac. Sci. Technol., B8, 495–498. P. S. Ho and T. Kwok, 1989, Electromigration in metals. Rep. Progr. Phys., 52, 301–347. M. Hommel, A. H. Fischer, A. v. Glasow and A. E. Zitzelsberger, 2001, Stress-induced voiding in aluminum and copper interconnects. In: ‘‘6th International Workshop on Stress-induced Phenomena in Metallization,’’ eds. S. P. Baker, M. A. Korhonen, E. Arzt and P. S. Ho, Am. Inst. Phys., pp. 157–168. 59 J. K. Howard, J. F. White and P. S. Ho, 1978, Intermetallic compounds of Al and transitions metals: effect of electromigration in 12-mm-wide lines. J. Appl. Phys., 49, 4083–4093. K. J. Hsia, Z. Suo and W. Yang, 1994, Cleavage due to dislocation conﬁnement in layered materials. J. Mech. Phys. Solids, 42, 877–896. C.-K. Hu, L. Gignac, S. G. Malhotra and R. Rosenberg, 2001, Mechanisms for very long electromigration lifetime in dual-damascene Cu interconnections. Appl. Phys. Lett., 78, 904–906. C.-K. Hu, K. P. Rodbell, T. D. Sullivan, K. Y. Lee and D. P. Bouldin, 1995, Electromigration and stress-induced voiding in ﬁne Al and Al-alloy thin-ﬁlm lines. IBM J. Res. Develop., 39, 465–497. C.-K. Hu, R. Rosenberg and K. Y. Lee, 1999, Electromigration path in Cu thin-ﬁlm lines. Appl. Phys. Lett., 74, 2945–2947. C.-K. Hu, M. B. Small and P. S. Ho, 1993, Electromigration in Al(Cu) two-level structures: effect of Cu and kinetics of damage formation. J. Appl. Phys., 74, 969– 978. M. S. Hu and A. G. Evans, 1989, The cracking and decohesion of thin ﬁlms on ductile substrates. Acta Metall., 37, 917–925. M. Huang, Z. Suo and Q. Ma, 2001, Metal ﬁlm crawling in interconnect structures caused by cyclic temperatures. Acta Mater., 49, 3039–3049. M. Huang, Z. Suo and Q. Ma, 2002, Ratcheting induced cracks in thin ﬁlm structures. J. Mech. Phys. Solids, 50, 1079–1098. M. Huang, Z. Suo, Q. Ma and H. Fujimoto, 2000, Thin ﬁlm cracking and ratcheting caused by temperature cycling. J. Mater. Res., 15, 1239–1242. R. Huang, J. H. Prévost, Z. Y. Huang and Z. Suo, 2003, Channel-cracking of thin ﬁlms with the extended ﬁnite element method, submitted. H. B. Huntington and A. R. Grone, 1961, Current-induced marker motion in gold wires. J. Phys. Chem. Solids, 20, 76–87. J. W. Hutchinson and A. G. Evans, 2000, Mechanics of materials: top-down approaches to fracture. Acta Mater., 48, 125–135. J. W. Hutchinson and Z. Suo, 1991, Mixed-mode cracking in layered materials. Adv. Appl. Mech., 29, 63–191. M. Isagawa, Y. Iwasaki and T. Sutoh, 1980, Deformation of Al metallization in plastic encapsulated semiconductor devices caused by thermal shock. In: ‘‘Proc. Int. Reliability Phys. Symp.,’’ pp. 171–177. S. Jansson and F. A. Leckie, 1992, Mechanical-behavior of a continuous ﬁber-reinforced aluminum matrix composite subjected to transverse and thermal loading. J. Mech. Phys. Solids, 40, 593–612. R. E. Jones and M. L. Basehore, 1987, Stress analysis of encapsulated ﬁne-line aluminum interconnect. Appl. Phys. Lett., 50, 725–727. A. M. Karlsson and A. G. Evans, 2001, A numerical model for the cyclic instability of thermally grown oxides in thermal barrier systems. Acta Mater., 49, 1793–1804. R. R. Keller, J. A. Nucci and D. P. Field, 1997, Local textures and grain boundaries in voided copper interconnects. J. Electron. Mater., 26, 996–1001. S.-Y. Kook and R. H. Dauskardt, 2002, Moisture-assisted subcritical debonding of a polymer/metal interface. J. Appl. Phys., 91, 1293–1303. M. A. Korhonen, R. D. Black and C.-Y. Li, 1991, Stress relaxation of passivated aluminum line metalizations on silicon substrate. J. Appl. Phys., 69, 1748–1755. M. A. Korhonen, P. Borgesen, K. N. Tu and C.-Y. Li, 1993, Microstructure based statistical model of electromigration damage in conﬁned line metallizations in the presence of thermally induced stresses. J. Appl. Phys., 73, 3790–5004. bib48 bib49 bib50 bib51 bib52 bib53 bib54 bib55 bib56 bib57 bib58 AU:14 bib59 bib60 bib61 bib62 AU:15 bib63 bib64 bib65 bib66 bib67 bib68 bib69 CSI : 08125 60 bib70 bib71 AU:16 bib72 bib73 bib74 bib75 AU:17 bib76 bib77 bib78 AU:18 bib79 AU:18 bib80 bib81 bib82 bib83 bib84 bib85 bib86 bib87 bib88 bib89 AU:19 bib90 Reliability of Interconnect Structures O. Kraft and E. Arzt, 1997, Electromigration mechanisms in conductor lines: void shape changes and slit-like failure. Acta Mater., 45, 1599–1611. M. Lane, R. H. Dauskardt, A. Vainchtein and H. Gao, 2000, Plasticity contributions to interface adhesion in thin ﬁlm interconnect structures. J. Mater. Res., 15, 2758–2769. M. Lane, R. H. Dauskardt, N. Krishna and I. Hashim, 2000, Adhesion and reliability of copper interconnects with Ta and TaN barrier layers. J. Mater. Res., 15, 203– 211. J. Lau, C. P. Wong, J. L. Prince and W. Nakayama, 1998, ‘‘Electronic Packaging, Design, Materials, Process, and Reliability,’’ McGraw-Hill, New York. B. Lawn, 1993, ‘‘Fracture of Brittle Solids,’’ Cambridge University Press, Cambridge. K.-D. Lee, X. Lu, E. T. Ogawa, H. Matsuhashi and P. S. Ho, 2002, Electromigration study of Cu/low k dualdamascene interconnects. In: ‘‘40th Ann. Proc. IEEE Int. Reliability Phys. Symp.,’’ pp. 322–326. K. L. Lee, C.-K. Hu and K. N. Tu, 1995, In situ scanning electron microscope comparison studies on electromigration of Cu and Cu(Sn) alloys for advanced chip interconnects. J. Appl. Phys., 78, 4428–4437. F. Z. Li, C. F. Shih and A. Needleman, 1985, A comparison of methods for calculating energy release rates. Eng. Fract. Mech., 21, 405–421. J. Liang, R. Huang, J. H. Prévost and Z. Suo, 2002a, Concomitant thin ﬁlm cracking and underlayer creep, Exp. Mech., submitted. J. Liang, R. Huang, J. H. Prévost and Z. Suo, 2002b, Evolving crack patterns in thin ﬁlms with the extended ﬁnite element method, Int. J. Solids Struct., submitted. K. M. Liechti and Y. S. Chai, 1991, Biaxial loading experiments for determining interfacial fracture-toughness. J. Appl. Mech., 58, 680–687. E. Liniger, L. Gignac, C.-K. Hu and S. Kaldor, 2002, In situ study of void growth kinetics in electroplated Cu lines. J. Appl. Phys., 92, 1803–1810. X. H. Liu, Z. Suo, Q. Ma and H. Fujimoto, 2000, Cracking and debonding in integrated circuit structures. Eng. Fract. Mech., 66, 387–402. T. C. Lu, J. Yang, Z. Suo, A. G. Evans, R. Hecht and R. Mehrabian, 1991, Matrix cracking in intermetallic composites caused by thermal expansion mismatch. Acta Metall. Mater., 39, 1883–1890. Q. Ma, S. Chiras, D. R. Clarke and Z. Suo, 1995, High resolution determination of the stress in individual interconnect lines and the variation due to electromigration. J. Appl. Phys., 78, 1614–1622. Q. Ma, J. Xie, S. Chao, S. El-Mansy, R. McFadden and H. Fujimoto, 1998, Channel cracking technique for toughness measurement of brittle dielectric thin ﬁlms on silicon substrates. Mater. Res. Soc. Symp. Proc., 516, 331–336. S. X. Mao and A. G. Evans, 1997, The inﬂuence of blunting on crack growth at oxide/metal interfaces. Acta Mater., 45, 4263–4270. T. Marieb, P. Flinn, J. C. Bravman, D. Gardner and M. Madden, 1995, Observations of electromigration induced void nucleation and growth in polycrystalline and near-bamboo passivated Al lines. J. Appl. Phys., 78, 1026–1032. S. J. Martin, J. P. Godschalx, M. E. Mills, E. O. Shaffer and P. H. Townsend, 2000, Development of a lowdielectric-constant polymer for the fabrication of integrated circuit interconnect. Adv. Mater., 12, 1769–1778. P. P. L. Matos, R. M. McMeeking, P. G. Charalambides and M. D. Drory, 1989, A method for calculating stress intensities in bimaterial fracture. Int. J. Fract., 40, 235– 254. J. W. McPherson and C. F. Dunn, 1987, A model for stress-induced notching and voiding in very large-scale integrated Al–Si (1%) metalization. J. Vac. Sci. Techol., B5, 1321–1325. S. Michaelides and S. K. Sitaraman, 1999, Die cracking and reliable die design for ﬂip-chip assemblies. IEEE Trans. Adv. Packag., 22(4), 602–613. N. Moes, J. Dolbow and T. Belytschko, 1999, A ﬁnite element method for crack growth without remeshing. Int. J. Numerical Methods in Eng., 46, 131–150. M. Morgen, E. T. Ryan, J.-H. Zhao, C. Hu, T. Cho and P. S. Ho, 1999, Low dielectric constant materials for advanced interconnects. JOM, 37–40. A. Needleman and E. Van der Giessen, 2001, Discrete dislocation and continuum descriptions of plastic ﬂow. Mater. Sci. Eng., A309, 1–13. W. D. Nix, 1989, Mechanical-properties of thin-ﬁlms. Metall. Trans., 20A, 2217–2245. E. T. Ogawa, J. W. McPherson, J. A. Rosal, K. J. Dickerson, T.-C. Chiu, L. Y. Tsung, M. K. Jain, T. D. Boniﬁeld, J. C. Ondrusek and W. R. McKee, 2002, Stress-induced voiding under vias connected to wide Cu metal leads. Proceedings of 2002 IEEE International Reliability Physics Symposium. T. S. Oh, R. M. Cannon and R. O. Ritchie, 1987, Subcritical crack-growth along ceramic-metal interfaces. J. Am. Ceram. Soc., 70, C352–C355. H. Okabayashi, 1993, Stress-induced void formation in metallization for integrated circuits. Mater. Sci. Eng., R11, 191–241. T. R. Reid, 1984, ‘‘The Chip,’’ Simon & Shuster, New York. I. E. Reimanis, B. J. Dalgleish and A. G. Evans, 1991, The fracture-resistance of a model metal ceramic interface. Acta Metall. Mater., 39, 3133–3141. J. R. Rice, 1988, Elastic fracture mechanics concepts for interfacial cracks. J. Appl. Mech., 55, 98–103. J. E. Rim, F. Shi, D.-I. Lee, F. Ohta and R. H. Dauskardt, 2002, Adhesion and debonding of low-k carbon-doped oxide ﬁlms in multi-layer thin ﬁlm structures. J. Mater. Res., submitted. J. H. Rose, 1992, Fatal electromigration voids in narrow aluminum–copper interconnect. Appl. Phys. Lett., 61, 2170–2172. R. Rosenberg, D. C. Edelstein, C.-K. Hu and K. P. Rodbell, 2000, Copper metallization for high performance silicon technology. Ann. Rev. Mater., 30, 229–262. J. E. Sanchez, L. T. McKnelly and J. W. Morris, 1992, Slit morphology of electromigration induced open circuit failures in ﬁne line conductors. J. Appl. Phys., 72, 3201– 3203. A. I. Sauter and W. D. Nix, 1992, A study of stress-driven diffusive growth of voids in encapsulated interconnect lines. J. Mater. Res., 7, 1133–1143. A. Sekiguchi, J. Koike, S. Kamiya, M. Saka and K. Maruyama, 2001, Void formation by thermal stress concentration at twin interfaces in Cu thin ﬁlms. Appl. Phys. Lett., 79, 1264–1266. E. O. Shaffer, F. J. Mcgarry and L. Hoang, 1996, Designing reliable polymer coatings. Polym. Eng. Sci., 36, 2375–2381. T. M. Shaw, L. Gignac, X.-H. Liu, R. R. Rosenberg, E. Levine, P. Mclaughlin, P.-C. Wang, S. Greco and G. Biery, 2001, Stress voiding in wide copper lines. In: ‘‘6th International Workshop on Stress-induced Phenomena in Metallization,’’ eds. S. P. Baker, M. A. Korhonen, E. Arzt and P. S. Ho, Am. Inst., Phys., pp. 177–183. Y. L. Shen, S. Suresh, M. Y. He, A. Bagchi, O. Kienzle, M. Ruhle and A. G. Evans, 1998, Stress evolution in passivated thin ﬁlms of Cu on silica substrates. J. Mater. Res., 13, 1928–1937. C. F. Shih, R. J. Asaro and N. P. O’Dowd, 1991, Elastic– plastic analysis of cracks on bimaterial interfaces: 3. Large-scale yielding. J. Appl. Mech., 58, 450–463. bib91 bib92 bib93 AU:20 bib94 bib95 bib96 AU:21 bib97 bib98 bib99 bib100 bib101 bib102 AU:22 bib103 bib104 bib105 bib106 bib107 bib108 bib109 AU:23 bib110 bib111 CSI : 08125 Electromigration bib112 AU:24 bib113 bib114 bib115 bib116 bib117 bib118 bib119 bib120 bib121 bib122 bib123 bib124 bib125 bib126 bib127 AU:25 61 J. M. Snodgrass, D. Pantelidis, M. L. Jenkins, J. C. Bravman and R. H. Dauskardt, 2002, Subcritical debonding of polymer/silica interfaces under monotonic and cyclic fatigue loading. J. Mater. Res., submitted. E. Suhir, 2002, Accelerated life testing (ALT) in microelectronics and photonics: its role, attributes, challenges, pitfalls, and interaction with qualiﬁcation tests. J. Electron. Packag., 124, 281–291. T. D. Sullivan, 1996, Stress-induced voiding in microelectron metallization: void growth models and reﬁnements. Ann. Rev. Mater. Sci., 26, 333–364. S. Suresh, 1998, ‘‘Fatigue of Materials,’’ 2nd edn, Cambridge University Press, Cambridge. B. Sun, Z. Suo and A. G. Evans, 1994, Emergence of crack by mass transport in elastic crystals stressed at high temperatures. J. Mech. Phys. Solids, 42, 1653–1677. Z. Suo, 1998, Stable state of interconnect under temperature change and electric current. Acta Mater., 46, 3725– 3732. Z. Suo and J. He, 2002, Unpublished research. Z. Suo and J. W. Hutchinson, 1989, Sandwich specimens for measuring interface crack toughness. Mater. Sci. Eng., A107, 135–143. Z. Suo and J. W. Hutchinson, 1990, Interface crack between two elastic layers. Int. J. Fract., 43, 1–18. Z. Suo, C. F. Shih and A. G. Varias, 1993, A theory for cleavage cracking in the presence of plastic ﬂow. Acta Metall. Mater., 41, 1551–1557. H. Tada, P. C. Paris and G. R. Irwin, 1985, ‘‘The Stress Analysis of Cracks Handbook,’’ Del Research, St. Louis, MO. R. E. Thomas, 1985, Stress-induced deformation of aluminum metallization in plastic molded semiconductor-devices. IEEE Trans. Compon. Hybrids Manuf. Technol., 8, 427–434. M. D. Thouless, 1991, Cracking and delamination of coatings. J. Vac. Sci. Technol., A9, 2510–2515. M. D. Thouless, A. G. Evans, M. F. Ashby and J. W. Hutchinson, 1987, The edge cracking and spalling of brittle plates. Acta Metall., 35, 1333–1341. M. D. Thouless, H. H. Yu, Z. J. Zhao and W. Yang, 1996, Damage nucleation during electromigration along an isolated interface in an elastic medium. J. Mech. Phys. Solids, 44, 371–387. S. P. Timoshenko and J. N. Goodier, 1970, ‘‘Theory of Elasticity,’’ McGraw-Hill. T. Turner and K. Wendel, 1985, The inﬂuence of stress on aluminum conductor life. In: ‘‘23rd Ann. Proc. IEEE Int. Reliability Phys. Symp.,’’ pp. 142–147. S. Vaidya, T. T. Sheng and A. K. Sinha, 1980, Linewidth dependence of electromigration in evaporated Al0.5%Cu. Appl. Phys. Lett., 36, 464–466. A. G. Varias, Z. Suo and C. F. Shih, 1991, Ductile failure of a constrained metal foil. J. Mech. Phys. Solids, 39, 963–986. R. P. Vinci and S. P. Baker (eds.), 2002, Mechanical Properties in Small Dimensions. MRS Bull., 27, 12–53. A. A. Volinsky, N. R. Moody and W. W. Gerberich, 2002, Interfacial toughness measurements for thin ﬁlms on substrates. Acta Mater., 50, 441–466. J. S. Wang and Z. Suo, 1990, Experimental determination of interfacial toughness curves using Brazil-nut-sandwiches. Acta Metall., 38, 1279–1290. P.-C. Wang, G. S. Cargill, I. C. Noyan and C.-K. Hu, 1998, Electromigration-induced stress in aluminum conductor lines measured by x-ray microdiffraction. Appl. Phys. Lett., 72, 1296–1298. P.-C. Wang and R. G. Filippi, 2001, Electromigration threshold in copper interconnects. Appl. Phys. Lett., 78, 3598–3600. W. Wang, Z. Suo and T.-H. Hao, 1996, A simulation of electromigration-induced transgranular slits. J. Appl. Phys., 79, 2394–2403. X. Yan and R. K. Agarwal, 1998, Two test specimens for determining the interfacial fracture toughness in ﬂip-chip assemblies. ASME Trans. J. Electron. Packag, 120, 150– 155. T. Ye, Z. Suo and A. G. Evans, 1992, Thin ﬁlm cracking and the roles of substrate and interface. Int. J. Solids Struct., 29, 2639–2648. H. H. Yu, M. Y. He and J. W. Hutchinson, 2001, Edge effects in thin ﬁlm delamination. Acta Mater., 49, 93– 107. J. Yue, W. Funsten and R. Tayler, 1985, Stress induced voids in aluminum interconnects during IC processing. In: ‘‘23rd Ann. Proc. IEEE Int. Reliability Phys. Symp.,’’ pp. 126–134. Z. C. Xia and J. W. Hutchinson, 2000, Crack patterns in this ﬁlms. J. Mech. Phys. Solids, 48, 1107–1131. Y. W. Zhang, A. F. Bower, L. Xia and C. F. Shih, 1999, Three dimensional ﬁnite element analysis of the evolution of voids and thin ﬁlms by strain and electromigration induced surface diffusion. J. Mech. Phys. Solids, 47, 173–199. Copyright 2002, Elsevier Science Ltd. All Rights Reserved No part of this publication may be reproduced, stored in any retrieval system or transmitted in any form or by any means: electronic, electrostatic, magnetic tape, mechanical, photocopying, recording or otherwise, without permission in writing from the publishers. Comprehensive Structural Integrity ISBN (set): 0-08 0437494 Volume 8; (ISBN: 0-080441513); pp. 1–61 bib128 AU:26 bib129 bib130 bib131 bib132 bib133 bib134 bib135 bib136 bib137 bib138 bib139 bib140 AU:27 bib141 bib142